Modeling and Analysis of Nuclear Fuel Pin Behavior for Innovative Lead Cooled FBR. L. Luzzi, S. Lorenzi, D. Pizzocri, D. Rozzia, A. Aly, A.


 Amy Sheena Tucker
 1 years ago
 Views:
Transcription
1 Inserire logo o denominazione del cobeneficiario Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DEO SVIUPPO ECONOMICO Modeling and Analysis of Nuclear Fuel Pin Behavior for Innovative ead Cooled FBR. uzzi, S. orenzi, D. Pizzocri, D. Rozzia, A. Aly, A. Del Nevo Report RdS/PAR213/22
2 Modeling and Analysis of Nuclear Fuel Pin Behavior for Innovative ead Cooled FBR. uzzi, S. orenzi, D. Pizzofri  CIRTEN POIMI, D. Rozzia, A. Aly, A. Del Nevo  ENEA Settembre 214 Report Ricerca Sistema Elettrico Accordo Programma Ministero dello Sviluppo Economico  ENEA Piano Annuale Realizzazione 213 Area: Produzione energia elettrica e protezione dell'ambiente Progetto: Sviluppo competenze scientifiche nel campo della sicurezza nucleare e collaborazione ai programmi internazionali per il nucleare IV Generazione Obiettivo: Sviluppo competenze scientifiche nel campo della sicurezza nucleare Responsabile del Progetto: Mariano Tarantino, ENEA Il presente documento descrive le attività ricerca svolte all interno dell Accordo collaborazione "Sviluppo competenze scientifiche nel campo della sicurezza e collaborazione ai programmi internazionali per il nucleare IV generazione" Responsabile scientifico ENEA: Mariano Tarantino Responsabile scientifico CIRTEN: Giuseppe Forasassi
3
4 Sigla identificazione ADPFISS P (This page has been intentionally left blank)
5 Sigla identificazione ADPFISS P CIRTEN Consorzio Interuniversitario per la Ricerca TEcnologica Nucleare POITECNICO DI MIANO DIPARTIMENTO DI ENERGIA, Sezione INGEGNERIA NUCEARE  CeSNEF Part1 Modeling and analysis of nuclear fuel pin behavior for innovative lead cooled FBR elio uzzi, Stefano orenzi, Davide Pizzocri CERSEPOIMI R 1493/213 Milano, Agosto 214 avoro svolto in esecuzione dell Attività P2.A.3_A AdP MSEENEA sulla Ricerca Sistema Elettrico  Piano Annuale Realizzazione 213 Progetto B.3.1 "Sviluppo competenze scientifiche nel campo della sicurezza nucleare e collaborazione ai programmi internazionali per il nucleare IV generazione"
6 Sigla identificazione ADPFISS P (this page is intentionally left blank)
7 Sigla identificazione ADPFISS P IST OF CONTENTS 1 INTRODUCTION EAD AS A COOANT IN FAST REACTORS General considerations Heat exchange correlation for Nusselt number Corrosion of the cladng Other relevant properties of lead AUSTENITIC STAINESS STEES FOR EADCOOED FAST REACTORS Thermophysical properties Mechanical properties Swelling Thermal creep strain rate Cumulative Damage Function Irraation creep CONCUSION AND FUTURE WORK... 38
8 Sigla identificazione ADPFISS P (this page is intentionally left blank)
9 Sigla identificazione ADPFISS P Introduction The eadcooled Fast Reactor (FR) has been selected by the Generation IV International Forum as one of the candates for the next generation of nuclear power plants (GIF, 22). Advanced reactor concepts cooled by Heavy iquid Metals (HMs) ensure a great potential for plant simplifications and higher operating efficiencies compared to other coolants, nevertheless introducing adtional safety concerns and design challenges (Cacuci, 21). Reactor contions of HMcooled reactor designs (e.g., extended exposure to neutron irraation, high temperature, corrosive environment) impose challenges for engineers and designers concerning the selection of structural and cladng materials. Key guidance on material behavior and help to improve the design can be achieved by means of fuel pin performance codes. Since the fuel pin behavior is determined by the synergy of several phenomena (heat transfer to the coolant, creep, swelling and corrosion of the cladng, relocation, densification, creep, and swelling of the fuel, fission gas release, etc.), a fuel pin analysis can be adequately accomplished by means of integral performance codes. In the present work, the TRANSURANUS code (assmann et al., 213) developed at JRCITU (Karlsruhe) has been extended for the analysis of nuclear fuel pin behavior of the FR employing 1515Ti austenitic steels as cladng material. This work is grafted in the research activity of the Nuclear Reactor Group of the Politecnico Milano on FRs. The particular features of this innovative reactor concepts attained the attention of the European Commission and the EADER Project (Ead Advanced DEmonstration Reactor) has been introduced in the 7th Framework Program (FP7 As a part of the EADER Project, the design of a demonstrator reactor is forecasted. This is a small (3 MWth) reactor called AFRED (Advanced eadcooled Fast Reactor) whose aim is to prove the technical and economic feasibility of the Generation IV lead reactor concept (Alemberti et al., 213). The 1515Ti austenitic steel is considered to be the cladng material in the AFRED reactor, as well as for other fast reactor systems like the AcceleratorDriven System MYRRHA (Aït Abderrahim et al., 212) and the Soum Fast Reactor ASTRID (Gavoille et al., 213). Despite the lower resistance to void swelling compared to the ferriticmartenstic steel T91 (the former candate material for the cladng), the 1515Ti austenitic steel has been selected due to the better thermal creep resistance, the good mechanical strength and because it has been already qualified and licensed in fast reactors. This report presents a critical review of the main FR material properties (except for the fuel, which is out of the scope of the present deliverable), aimed at the extension and validation of the fuel pin performance code TRANSURANUS (TU) for modeling and analyzing the fuel pin integral behavior in innovative FRs, specifically referring to the AFRED reactor. Actually, an FRoriented version of TRANSURANUS represents the first, necessary step in a more general process of analysis and optimization (see Figure 1), finalized to support the design and the construction of AFRED by means of the following actions: i) critical analysis of the fuel pin behavior in reactor through the study of a "reference case" (based on "best estimate" models) to verify the respect of design limits; ii) identification of possible critical issues through an extensive sensitivity analysis on the most significant phenomena (both in normal operation and accident contions) affected by a considerable modeling uncertainty, and oriented to the definition of a "worst case scenario" for the fuel pin performance;
10 Sigla identificazione ADPFISS P Part I FRoriented TU extension Part II safetyoriented pin design feedbacks AFRED reference case sensitivity analysis and worst case Figure 1: Scheme of the optimization process that can be carried out by means of the extended TRANSURANUS version to give feedbacks on the AFRED conceptual design. iii) iv) optimization of the fuel pin design, in order to improve the performance and safetybydesign features of the AFRED reactor; identification of design solutions aimed at achieving enlarged safety margins and of the most adequate FA geometrical configuration from the thermomechanical point of view (e.g., optimization of the raal power peak factor in the reactor core). The v1m3j12 version of the TRANSURANUS code has to be considered as the starting point of the work, which has permitted the development of an FRoriented version that includes an updating of the correlations for the thermophysical properties of the lead and introduces new correlations for swelling, thermal creep and heat capacity of the 1515Ti austenitic steels. As first step of this process, a review of the main properties of lead as a coolant is carried out, making a comparison with literature data. Afterwards, a critical review of the correlations for the 1515Ti austenitic steels is performed. In this report, on the basis of the information available in literature, the correlations included in the FRoriented version of TRANSURANUS, for evaluating the thermophysical properties of lead, the thermomechanical properties and the treatment of the inreactor behavior of 1515Ti steels, are reported.
11 Sigla identificazione ADPFISS P IST OF SYMBOS atin symbols A, B, C materials constants c p specific heat (at constant pressure) [J kg 1 K 1 ] CDF cladng cumulative damage function [] D pin ameter [m] E Young s modulus [GPa] mean neutron energy [MeV] EAB elongation at break [%] MP arsonmiller Parameter Nu Nusselt number [] Nu lam laminar Nusselt number (Ushakov correlation) [] p pin pitch [m] P P parameter (thermal creep) Pe Peclet number [] R perfect gas constant [cal mol 1 K 1 ] t temperature [ C] t R rupture time [h] T temperature [K] T boil boiling temperature [K] T l liquidus temperature [K] T melt melting temperature [K] T s solidus temperature [K] Greek symbols ΔH specific activation energy [cal mol 1 ] Δt time interval [h] volume swelling strain [%] ε equivalent thermal creep strain [%] equivalent creep strain rate [% h 1 ] ε th equivalent thermal creep cladng hoop strain [%] ε th,r equivalent thermal creep cladng rupture strain [%] λ thermal conductivity [W m 1 K 1 ] ρ density [kg m 3 ] ρ density at 2 C [kg m 3 ] stress (Von Mises equivalent) [MPa] σ UT σ Y,.2% ultimate tensile strength [MPa] yield strength [MPa] fast neutron flux [n cm 2 s 1 ] Φ fast neutron fluence [1 22 ] ζ linear thermal expansion coefficient [%] ω Ushakov correlation parameter [] Δ incates variations
12 Sigla identificazione ADPFISS P IST OF ACRONYMS AIM AFRED ASTRID CEA CDF FA FAE FBR(s) FP7 GESA GIF HM IN ITU JOG JRC EADER FR(s) MFR(s) MP MYRRHA MOX NEA OECD P PCMI PD POIMI POITO SFR TU UT YS Austenitic Improved Material Advanced eadcooled Fast Reactor European Demonstrator Advanced Soum Technological Reactor for Industrial Demonstration Commisariat à l Energie Atomique Cumulative Damage Function Fuel Assembly Fuel Adjacency Effect Fast Breeder Reactor(s) 7 th Framework Program Gepulste ElektronenStrahlAnlage Generation IV International Forum Heavy iquid Metals Idaho National aboratory Institute for TransUranium elements Joint OxideGain Joint Research Center eadcooled European Advanced DEmonstration Reactor eadcooled Fast Reactor(s) iquid Metalcooled Fast Reactor(s) arsonmiller Parameter Multipurpose hybrid Research Reactor for Hightech Applications Mixed OXyde Nuclear Energy Agency Organization for Economic Cooperation and Development Parameter, cladng thermal creep Pellet Cladng Mechanical Interaction Pulsed aser Deposition Politecnico Milano Politecnico Torino Soum Fast Reactor(s) TRANSURANUS Ultimate Tensile strength Yield Strength
13 Sigla identificazione ADPFISS P IST OF FIGURES Figure 1: Scheme of the optimization process that can be carried out by means of the extended TRANSURANUS version to give feedbacks on the AFRED conceptual design Figure 2: Nusselt number dependence on Peclet number and on pitch parameters for liquid pure lead in a triangular lattice (far from spacers) accorng to simplified Ushakov correlation. The three curves are plotted with p/d = 1.3, 1.35 and Figure 3: iquid lead density (OECDNEA, 27) Figure 4: Gurvich correlation for isobaric specific heat of liquid lead as presented in OECDNEA (27) Figure 5: iquid lead thermal conductivity (OECDNEA, 27) Figure 6: Comparison between the Rudtsch et al. (25) data for linear thermal expansion and the correlation implemented in TRANSURANUS Figure 7: Comparison between the Rudtsch et al. (25) data for density and the correlation implemented in TRANSURANUS Figure 8: Specific heat correlation compared with recent experimental data for steel (Rudtsch et al., 25) Figure 9: Comparison between correlation and experimental data for thermal conductivity of a Ti stabilized 2% cold worked austenitic stainless steel Figure 1: Comparison between correlation and experimental data for the elastic modulus of 1515Ti stainless steel Figure 11: Correlations for ultimate tensile strength (UT) and yield strength (YS) are here plotted together Figure 12: The mismatch between correlation and open literature data for the rupture strain of the 1515Ti austenitic stainless steel is here clearly shown Figure 13: Comparison between experimental data and the "Specific AIM1" and "Generalized 1515Ti" correlations for the cladng steel swelling as a function of temperature Figure 14: Comparison between experimental data and the "Specific AIM1" and "Generalized 1515Ti" correlations for the cladng steel swelling as a function of dpa Figure 15: Többe correlation for the thermal creep strain rate of 1.497m steel Figure 16: Mofied Többe correlation for the thermal creep strain of the AIM1 steel. The fit is made on Gavoille data, Filacchioni data are reported for comparison Figure 17: P/stress correlation for 1.497m steel. Rupture time is calculated from equivalent stress, at fferent temperatures Figure 18: MP/stress correlation for AIM
14 Sigla identificazione ADPFISS P IST OF TABES Table 1: iquid lead density correlation Table 2: iquid lead specific heat capacity correlation Table 3: iquid lead thermal conductivity correlation Table 4: Chemical composition of some austenitic stainless steels of the 1515Ti family. Compositions are expressed in weight percentage [wt. %] (Gavoille et al., 213; Banerjee et al., 27) Table 5: 1515Ti steels linear thermal expansion correlation Table 6: 1515Ti steels specific heat correlation Table 7: 1515Ti steels thermal conductibility correlations Table 8: 1515Ti steels Young's modulus correlation Table 9: 1515Ti steels yield strength and ultimate tensile strength correlations Table 1: 1515Ti steels elongation at break correlations Table 11: 1.497m thermal creep strain rate correlation Table 12: AIM1 thermal creep strain rate correlation Table 13: Cumulative Damage Function (CDF) possible definitions Table 14: 1515Ti steels irraation creep correlation
15 Sigla identificazione ADPFISS P ead as a coolant in fast reactors In this section, the properties of lead are presented, focusing in particular on its use as a coolant in fast reactors. The OECDNEA Handbook (OECDNEA, 27) has been used as summarized and reasoned reference. 2.1 General considerations Pure lead is an interesting coolant in fast reactors due to its high mass number and its low absorption crosssection, which are fundamental properties for a fast reactor coolant. It has good thermal characteristics for heat removal. With respect to soum and leadbismuth eutectic (the other metals proposed as coolants in innovative MFRs), it has high melting temperature (327 C, 6 K) and an high boiling point (1749 C, 222 K) allowing a wide range of operation. Compared to soum, it does not present the problem of strong exothermic reaction with air and water, while with respect to the leadbismuth eutectic, it is less corrosive, it does not present the problem of activation issue typical of bismuth (polonium production) and does not present the issue of solification volume growth. Nevertheless, it is steelaggressive for the core materials both for erosion and corrosion issues (therefore, a flow velocity of less than 2 m s 1 is envisaged, and an oxygen control and/or a coating for cladng are required, respectively) and it is very toxic and polluting, requiring particular attention from production to sposal or recycling. 2.2 Heat exchange correlation for Nusselt number iquid lead is meant to be the coolant of FRs. Therefore, its heat exchange properties are fundamental. The heat exchange correlation has been developed by Ushakov et al. (1977) for regular hexagonal fuel elements, far from spacing grids. The correlation that is called in the TRANSURANUS routine is the following: ( ) ( ) (1) (1.3 < p/d < 2. in TU) In Figure 2, Ushakov correlation is plotted (Nu as a function of Pe) for three fferent pitch parameters (p/d = 1.3, 1.35 and 1.4). It should be noted that this correlation is just an approximation of the Ushakov complete correlation for triangular lattice, acceptable in the range of pinpitch over ameter incated above. The complete correlation is reported in Equation (2). ( ( ) ( ) ) ( ( ) ) (2)
16 Sigla identificazione ADPFISS P ( ) ( (( ) ) ) ( ) The complete correlation is implemented in TRANSURANUS, and called only when vality range for the simplified one. is out of the 3 Nu Pe Figure 2: Nusselt number dependence on Peclet number and on pitch parameters for liquid pure lead in a triangular lattice (far from spacers) accorng to simplified Ushakov correlation. The three curves are plotted with p/d = 1.3, 1.35 and Corrosion of the cladng Ushakov The problem of keeping a stainless steel in the aggressive environment represented by liquid lead is not yet solved, but certainly maintaining flow velocity under 2 m s 1 reduces the erosion effect. Nevertheless, the stainless steel of which the cladng is made requires further protection, and fferent coating layers are under development. Among the proposed solutions, the most promising are the FeCrAlY alloy, realized through the socalled GESA (Gepulste ElektronenStrahlAnlage) treatment (Weisenburger et al., 28) and the Al 2 O 3 coating realized through Pulse aser Deposition (PD) (Garcia Ferrè et al., 213) 1. For our purposes, the modeling solution that can be adopted is substitute an external layer of the cladng (4 μm) by a coating which is not affected by 1 The lead corrosion and erosion of the cladng is a critical issue for FR development. A complete review of this research field goes beyond the scope of this work.
17 Sigla identificazione ADPFISS P corrosion and is featured by a thermal conductivity of 16 W m 1 K 1 (Agosti et al., 213). Mechanical and irraation effects on the coating are presently not taken into account. 2.4 Other relevant properties of lead The other properties of liquid lead are less problematic for this work, and therefore they are simply reported with their correlation accorng to OECDNEA (27). Melting point OECDNEA (27) incates an interpolation value between the ones available in literature. The dependence on pressure is in the order of a.8 K increase per 1 MPa increase and thus it has been sregarded. Boiling point For boiling point, uncertainties are higher than for melting point. The value recommended in the OECDNEA (27) is the following: Density The density of liquid lead can be related to temperature with a simple linear correlation. Even if purity is not well specified in single references, agreement within data is very strong, with uncertainty under 1%. This is shown in Figure 3. The correlation is reported in Table 1. (3) (4) Table 1: iquid lead density correlation. [ ] [ ] Reference OECDNEA, 27 Correlation Figure 3: iquid lead density (OECDNEA, 27).
18 Sigla identificazione ADPFISS P Specific heat capacity at constant pressure Accorng to OECDNEA (27), Gurvich and Veyts (1991) correlation is suggested as a reasonable choice between available data (Table 2). Both data and correlation are plotted in Figure 4. Table 2: iquid lead specific heat capacity correlation. [ ] [ ] Reference OECDNEA, 27 Correlation Figure 4: Gurvich correlation for isobaric specific heat of liquid lead as presented in OECDNEA (27). Thermal conductivity The data regarng the thermal conductivity of liquid lead are very spersed. Therefore, in this case, the recommendation by OECDNEA (27) is particularly useful (Table 3). The proposed correlation is linear and fits well recent data, as is shown in Figure 5. Table 3: iquid lead thermal conductivity correlation. [ ] [ ] Reference OECDNEA, 27 Correlation
19 Sigla identificazione ADPFISS P Figure 5: iquid lead thermal conductivity (OECDNEA, 27).
20 Sigla identificazione ADPFISS P Austenitic stainless steels for eadcooled Fast Reactors This section presents the correlations for the main thermal and mechanical properties of 1515Ti austenitic stainless steels adopted as cladng material for some leadcooled fast nuclear reactors (e.g., AFRED, MYRRHA). Specific austenitic stainless steels have been developed to be used as cladng materials in fast reactors. The main advantages of these materials are their good thermal creep behavior and their excellent mechanical properties. The main issue for these materials is to resist swelling, avoing the risk of gap reopening during fuel life and hence the occurrence of the socalled "thermal feedback effect" (ombar, 26). This is achieved through the inclusion of titanium, whose little TiC precipitates are able to increase the incubation time of the phenomena interacting with the voids created by fast neutrons irraation. Also silicon seems to play an important role in contrasting swelling. Moreover, the presence of boron goes in the rection of improving creep ductility (Frost, 1994). The characteristics of these steels may justify their use as structural materials also for other components, such as the Fuel Assemblies (FAs) wrapper. Following this concept, a certain number of 1515Ti steels has been developed in fferent countries: D9 in the US, AIM1 in France, DIN in Germany. The chemical compositions of these alloys is summarized in Table 4. All these materials are cold worked at 2%. Table 4: Chemical composition of some austenitic stainless steels of the 1515Ti family. Compositions are expressed in weight percentage [wt. %] (Gavoille et al., 213; Banerjee et al., 27). C Cr Ni Mo Si Mn Ti Nb P B AIM DIN D In the following subsections, a review of the main properties of 1515Ti will be presented, all described by outofpile correlations. The properties of the austenitic steels (Többe, 1975) are compared with other literature data in order to assess their vality. On the other hand, the specific heat (Banejree, 27), the swelling and the thermal creep have been updated. In particular, these last two properties have been carefully evaluated since the fferent composition of the alloying material has a great impact on these material features. 3.1 Thermophysical properties Here below, the fundamental outofpile thermal properties of 1515Ti austenitic stainless steels are reported. For all these properties, the effect of specific alloyed elements is minimum, and therefore the fference between the specific alloys (AIM1, and D9) is practically negligible. On the other hand, for some mechanical properties, swelling and thermal creep, the fferent percentage of the alloying elements has a relevant impact on these properties. Melting temperature In the TRANSURANUS code, the melting temperature is set in the SOIMT subroutine at: T melt = 1673 K (5)
21 Sigla identificazione ADPFISS P From literature data, the melting temperature (liquidus) and solification temperature (solidus) have been measured for steel by Nikolopoulos and Schulz (1979). The values proposed in these references are: (6) inear thermal expansion The thermal expansion is here described by a strain parameter. The correlation implemented in TRANSURANUS is proposed by Gehr (1973). Table 5: 1515Ti steels linear thermal expansion correlation. [ ] [ ] Reference Gehr, 1973 Correlation In general, there is a good agreement between literature data, with no strong dependence on the chemical composition of the steel (around reference values) or on the thermomechanical process (cold working, aging). In Figure 6, the data reported in Rudtsch et al. (25) are compared with the correlation implemented in the FRoriented version. inear thermal expansion [] T [K] Rudtsch (25) TU Figure 6: Comparison between the Rudtsch et al. (25) data for linear thermal expansion and the correlation implemented in TRANSURANUS. Density The TRANSURANUS routine RO calculates the density of the steel as a function of temperature using the linear expansion correlation. The relation between these two quantities is straightforward: ( ) (7)
22 Sigla identificazione ADPFISS P Therefore, only the value at a certain reference temperature is needed. Equation (7) is implemented in TRANSURANUS (Schumann, 197), and results in good agreement with the value proposed by Rudtsch et al. (25). t = 2 [ C] (8) = 79 [kg m 3 ] An explicit fit for problems. is represented in Figure 7. This correlation does not present vality range 8 79 Density [kg m 3 ] T [K] Rudtsch (25) TU Figure 7: Comparison between the Rudtsch et al. (25) data for density and the correlation implemented in TRANSURANUS. Specific heat Specific heat measurements have been carried out in the range 2 1 C ( K). In Figure 8, the correlation proposed by Banerjee et al. (27) is compared with the data reported in Rudtsch et al. (25). The former correlation has been selected and implemented in the FRoriented version.
23 Sigla identificazione ADPFISS P Figure 8: Specific heat correlation compared with recent experimental data for steel (Rudtsch et al., 25). In Table 6, the correlation plotted in Figure 8 is reported. Table 6: 1515Ti steels specific heat correlation. [ ] [ ] Reference Banerjee, 27 Correlation c p = T T 2 Thermal conductivity The thermal conductivity of the cladng material is a fundamental property because it determines the temperature graent across the cladng, controlling thermal stress and temperature levels (which determine all the other mechanical properties). Therefore, it is fundamental to have a reliable correlation implemented in the routine AMBDA of TRANSURANUS code. It should be noticed that the cold work treatment slightly alters the thermal conductivity (especially over 9 K, region in which also the measurement uncertainty grows). Therefore, the degree of cold work should be specified. In Figure 9, the correlation proposed by Tobbe (1975) and implemented in the FRoriented version is reported and compared with the data from Rudtsch et al. (25) 2% cold worked steel. Table 7: 1515Ti steels thermal conductibility correlations. [ ] [ ] Reference Többe, 1975 Correlation
24 Sigla identificazione ADPFISS P Thermal conductivity [W m 1 K 1 ] T [K] TU Rudstch (25) Figure 9: Comparison between correlation and experimental data for thermal conductivity of a Ti stabilized 2% cold worked austenitic stainless steel. 3.2 Mechanical properties This subsection presents the most relevant mechanical properties of the 1515Ti austenitic stainless steels. Thermal creep and swelling phenomena will be treated separately. All the properties presented here are intended outofpile, therefore only the dependence on temperature is considered. The properties already implemented in the v1m3j12 version, and also adopted in the FRoriented version, will be scussed and compared with data and correlations found in literature, pointing out the critical issues. Young s modulus There are very few data available in the open literature about the Young s modulus of a 1515Ti steel (or about similar austenitic stainless steels). The only data found in literature come from Bergmann (1988) for steel. It is in general stated that the Young s modulus does not depend on the cold work degree. In Figure 1, the correlation proposed by Többe (1975) is plotted and compared with the data from Bergmann (1988). 22 Elastic modulus [GPa] T [K] TU Bergmann (1988) Figure 1: Comparison between correlation and experimental data for the elastic modulus of 1515Ti stainless steel.
25 Sigla identificazione ADPFISS P In Table 8, the correlation plotted in Figure 1 is reported. The range of vality should be the one explored in Bergmann experiment, 2 8 C ( K). Table 8: 1515Ti steels Young's modulus correlation. [ ] [ ] Reference Többe, 1975 Correlation The correlation implemented in TRANSURANUS overestimates the elastic modulus in all the range of temperatures. Yield strength and ultimate tensile strength These properties are scussed together because they represent the basic parameters of the stressstrain agram of a steel (along with rupture strain scussed in the next subsection and the Young s modulus). Moreover, it is important to notice that for these properties there is a quite strong sagreement between what reported in Filacchioni et al. (199) and what implemented in TRANSURANUS (Többe, 1975). The data reported in Filacchioni et al. (199) refer to the DS3, a 1515Ti austenitic steel close to the AIM1. The screpancies between the data and the correlation can be explained with the relevance of the alloying element for these properties. Accorngly, fferent steels of the 1515Ti family can show very fferent behavior. It is important to remind that every property has to be intended outofpile. Accorng to the literature data, measurements have been carried out until roughly 11 K ( 85 C) and therefore correlations are reliable until this temperature with around 1% of uncertainty. Nevertheless, the range of vality of these correlations is suitable for the fuel performance analysis of the FR in operational cases. Ultimate tensile strength Yield strength [MPa] T [K] TU UT TU YS Filacchioni (199) UT Filacchioni (199) YS Figure 11: Correlations for ultimate tensile strength (UT) and yield strength (YS) are here plotted together. In Table 9, the correlations plotted in Figure 11 are reported.
26 Sigla identificazione ADPFISS P Table 9: 1515Ti steels yield strength and ultimate tensile strength correlations. [ ] [ ] Reference Többe, 1975 Correlation T C T C T C if T 6 C Y,.2% T C 6 if 6 C T 1 C if T 1 C T C if T 6 C UT T C 6 if 6 C T 1 C if T 1 C The third segment of the correlation implemented in TRANSURANUS has a slope which is less than the second segment, bringing to higher values of ultimate tensile strength at high temperature, not supported by open literature data. Rupture strength is calculated from the rupture strain in TRANSURANUS, and therefore no specific correlation is implemented. Actually, also the rupture strain presents the same criticalities as the quantities described in this subsection. Rupture strain For the elongation at break it is fundamental to understand if the Többe (1975) data are reliable. There is sagreement between the correlation implemented in TRANSURANUS and the data proposed by Filacchioni et al. (199) on DS3, similar to AIM1. Once again, this behavior can be explained with the fferent composition of the alloying element that dramatically influences some properties. In adtion, this is the only property whose modeling in TRANSURANUS considers also the inpile behavior: when neutron fluence exceeds 1 22 n cm 2, the rupture strain is set at 6%. A conversion factor of n cm 2 = 1 dpa is assumed. In Figure 12, the correlations are plotted. In Table 1, the outofpile correlation plotted in Figure 12 is shown. Ropture strain [%] T [K] TU outofpile TU inpile Filacchioni (199) Figure 12: The mismatch between correlation and open literature data for the rupture strain of the 1515Ti austenitic stainless steel is here clearly shown.
27 Sigla identificazione ADPFISS P Correlation Table 1: 1515Ti steels elongation at break correlations. [ ] [ ] Reference Többe, Swelling Void swelling is a critical phenomenon for a cladng material to be used in a fast reactor. In particular, the risk of gap reopening and subsequent "thermal feedback" has to be avoided. Therefore, particular attention has been paid in adopting an austenitic stainless steel able to resist in an environment characterized by a fast neutron spectrum. Steels can be resistant to swelling in two ways: having long incubation time or having little swelling rates. In principle, swelling depends also on stress, because the stress field influences the stribution of raation induced point defects responsible of the phenomenon. A review of these effects can be found in Hübner (2). In order to implement swelling correlations in TRANSURANUS, it is necessary to consider both the dependence on temperature and the dependence on fast neutron fluence 2. In this work, the subroutine SWEOC has been updated with two correlations concerning two class of austenitic stainless steels. The first, called "Specific AIM1", refers to the most advanced steel irraated in Phénix (AIM1 austenitic stainless steel). The second, called "Generalized 1515Ti", refers to an older version of the steel. In Figure 13, both these correlations are plotted. "Specific AIM1" 2 V T( C) 49 % exp V (9) "Generalized 1515Ti" 2 V T( C) 45 % exp 2.5 V Φ is the fast neutron fluence vided by 1 22 n cm 2, while the conversion between fluence and dpa is (n cm 2 )/dpa. Accorng to the data plotted in Figure 14, it seems reasonable to assume a best estimate incubation time in the order of 6 dpa, while for the worst case a reasonable incubation time could be around 2 dpa. (1) 2 There is an intrinsic relation between the swelling and the creep phenomena. Different approaches to consider this interaction have been proposed (Hübner, 2), but they are not applied in the present work because of lack of data.
28 Sigla identificazione ADPFISS P Before reporting the correlations implemented in the TRANSURANUS, it must be said that screpancies in available data are very strong, that leads to the necessity of a sensitivity analysis for this important phenomenon. In any case, Dubuisson (213) and Bergmann et al. (23) are considered to be reliable data references. Swelling V/V (%) CEA incation 93 dpa "Specific AIM1" 93 dpa "Generalized Ti1515" 93 dpa 15 dpa 13 dpa 12 dpa 15 dpa 891 dpa 75 dpa 667 dpa 5 dpa 4 dpa dpa 13 dpa» dpa Temperature ( C) Figure 13: Comparison between experimental data and the "Specific AIM1" and "Generalized 1515Ti" correlations for the cladng steel swelling as a function of temperature. Swelling V/V (%) "Specific AIM1" 4 C "Specific AIM1" 55 C "Specific AIM1" 49 C "Generalized Ti1515" 5 C "Generalized Ti1515" 45 C 1515Ti BS Phenix Av. Phenix 6 C 575 C 55 C 53 C 5 C C 43 C 42 C 45 C 4 C Dose (dpa) Figure 14: Comparison between experimental data and the "Specific AIM1" and "Generalized 1515Ti" correlations for the cladng steel swelling as a function of dpa. 3.4 Thermal creep strain rate Thermal creep is a critical phenomenon for the cladng steel. The fferent chemical composition in terms of alloying elements plays a fundamental role in determining the creep strain rate of a steel.
29 Sigla identificazione ADPFISS P Therefore, in the FRoriented version two specific correlations for 1.497m and AIM1 steels have been included m creep strain rate For the 1.497m specific steel of the 1515Ti class, Többe (1975) correlation, already present in the v1m3j12 version, has been adopted in the FRoriented version for the thermal creep strain rate (Table 11). The structure of this correlation is a NabarroHerring equation, fferent from the typical Arrhenius equations used in creep strain rate modeling. In Figure 15, the correlation is plotted. Table 11: 1.497m thermal creep strain rate correlation. [ ] [ ] [ ] Reference % h 1 MPa K Többe, 1975 Correlation 1 Equivalent stress [MPa] 1 Tobbe 55 C Tobbe 65 C Tobbe 75 C 1 1.E6 1.E5 1.E4 1.E3 1.E2 1.E1 1.E+ Thermal creep equivalent strain rate [% h 1 ] Figure 15: Többe correlation for the thermal creep strain rate of 1.497m steel.
30 Sigla identificazione ADPFISS P AIM1 creep strain rate For the AIM1 specific steel of the 1515Ti class, a mofied version of the Többe correlation is adopted (Table 12), fitting Gavoille et al. (213) data. This correlation is implemented in the FRoriented version of TRANSURANUS. In Figure 16, the correlation is compared also with experimental data from Filacchioni et al. (199). Also this correlation presents a NabarroHerring structure. Table 12: AIM1 thermal creep strain rate correlation. [ ] [ ] [ ] Reference % h 1 MPa K Gavoille et al., 213 (data) Correlation E6 1.E5 1.E4 1.E3 1.E2 1.E1 1.E+ Equivalent stress [MPa] Thermal creep equivalents train rate [% h 1 ] Mod. Tobbe 55 C Mod. Tobbe 6 C Mod. Tobbe 65 C Mod.Tobbe 7 C Mod. Tobbe 75 C Mod. Tobbe 8 C Mod. Tobbe 85 C Filacchioni 75 C Filacchioni 55 C Filacchioni 65 C AIM1 55 C AIM1 6 C Figure 16: Mofied Többe correlation for the thermal creep strain of the AIM1 steel. The fit is made on Gavoille data, Filacchioni data are reported for comparison.
31 Sigla identificazione ADPFISS P Cumulative Damage Function In order to model the thermal creep behavior of the cladng steel, a Cumulative Damage Function (CDF) approach has been implemented in the FRoriented version of TRANSURANUS. A CDF is a creep failure criterion widely used and validated for a lot of fferent steels (Waltar et al., 211). In Table 13, two possible definitions are reported. If the value of CDF exceeds unity, it is assumed that the steel has accumulated an amount of strain which leads to rupture. In this work, a CDF defined with rupture time has been implemented in the FRoriented version. At each time step, thermal creep rupture time is calculated and the CDF value is proportionally increased. It is important to notice that the rupture time changes at each time step, depenng on the combination of stress and temperature in the cladng. In order to calculate the cladng CDF, the following process is applied: first of all, a parameter condensing temperature and rupture time (i.e., the arsonmiller parameter) is calculated from the equivalent (Von Mises) stress through an experimental correlation; secondly, the rupture time is calculated from the temperature through the condensed parameter; the rupture time is used to calculate the CDF increase. This process relies on the possibility of using just two relatively simple correlations to handle a phenomenon with three variables. One of these correlations is the definition of the condensed parameter, the other one is the stressparameter relation. Table 13: Cumulative Damage Function (CDF) possible definitions 3. Based on rupture time Based on rupture strain Definition of the arsonmiller Parameter (MP) The arsonmiller parameter definition derives from modeling the creep mechanism, by means of a threshold type equation. In particular, the creep rate temperature dependence can be expressed with an Arrhenius equation. Supposing that the dependence on temperature of the activation energy of the process is very little, the arsonmiller parameter can be defined as: (11) where is temperature in Kelvin, is a constant depenng on the material considered, and is the rupture time in hours. arsonmiller parameter is assumed to be function of the stress. This allows the use of this parameter to calculate rupture time from stress and temperature, which is fundamental in evaluating the CDF. The assumption of a low dependence of the activation energy on the temperature is not exactly verified. Therefore, other models have been developed for high temperature regime. Moreover, at high temperature, the physical microscopic phenomena which lead to creep are fferent, requiring a fferent modeling approach. A fferent parametric approach for 1515Ti steels The effort of introducing a new parameter is justified because the creep mechanism of the 1515Ti steels is not well described by an Arrhenius equation (Többe, 1975). The fference in the thermal 3 Accorng to Waltar et al. (211), a FAE (Fuel Adjacency Effect) coefficient can be added at the denominator, allowing for the chemical interaction between fuel and cladng (e.g., JOG formation). This interaction is neglected in the present work, because the mechanism of interaction between MOX fuel and austenitic cladng steel is still under investigation.
32 Sigla identificazione ADPFISS P creep mechanism should lead to the use of a fferent parameter. Indeed, arsonmiller parameter is by definition nonphysical for this class of steels. The creep mechanism of the 1515Ti steels can be described by means of a NabarroHerring equation (the same form of Többe correlation), which introduces a change in the creep behavior at high temperature. Two equations are in general used for NabarroHerring creep rate modeling, one being the approximation of the other: (12) In Equation (12), and are constants depenng on the material, is the perfect gas constant and represent the equivalent Von Mises stress applied to the material. The stress is involved in the creep mechanism because NabarroHerring thermal creep is interpreted by the migration of point defects in the metal lattice, which is governed by stress level. The hyperbolic sine term becomes important at high temperature. In analogy with the definition of arsonmiller parameter, from Equation (12) it is possible to define a parameter P merging temperature and rupture time as follows: ( ) (13) Comparing this result with arsonmiller parameter, it can be noticed how the presence of an high temperature effect is translated in a rescaling of the rupture time. In this subsection, both MP and P parameters are used to construct stressparameter agrams interpolating creep data of few stabilized austenitic stainless steels. What is expected is that, at high temperature and for steel of the 1515Ti class, P would be more reliable than MP. It is useful to summarize all the hypotheses made in the definition of P. Some of them are in common with arsonmiller parameter, some others are specific. 1) Creep rate can be modeled by a NabarroHerring equation (13). This means that the creep phenomenon has to be governed by pointlike entities (defects or little precipitates) in the lattice, at high temperature. 2) Activation energy of the creep phenomenon can be assumed independent of temperature and stress. 3) Stress variation effect is little compared with temperature effect. This is in general not true, particularly when strong stress graents are presents and creep is originated from vacancies flow. Hypothesis 3) is critical and should always be checked. In general, if stresses are intense, it is possible to go further in Mc aurin expansion, Equation (12), adng higher order terms. This results in a parameter that has the same functional structure of P, with more free parameters that have to be set.
33 Sigla identificazione ADPFISS P Rupture time correlation for 1.497m The thermal creep strain for 1.497m is calculated by means of Többe correlation, which has a NabarroHerring structure. This suggests that the correlation for rupture time should be based on P parameter. Indeed, a single stressmp correlation is not able to follow temperature changes. In Figure 17, the stressp correlation implemented in the FRoriented version of TRANSURANUS, based on Bergmann (1988) data, is reported. ( ) (14) (15) Rupture time [h] 1.E+1 1.E+9 1.E+8 1.E+7 1.E+6 1.E+5 1.E+4 1.E+3 1.E+2 1.E+1 1.E+ 1.E Equivalent stress [MPa] Bergmann K P/stress correlation Rupture time [h] 1.E+1 1.E+9 1.E+8 1.E+7 1.E+6 1.E+5 1.E+4 1.E+3 1.E+2 1.E+1 1.E+ 1.E Equivalent stress [MPa] Bergmann K P/stress correlation Figure 17: P/stress correlation for 1.497m steel. Rupture time is calculated from equivalent stress, at fferent temperatures.
34 Sigla identificazione ADPFISS P Rupture time correlation for AIM1 The thermal creep strain for AIM1 is calculated by means of the mofied Többe correlation, which has a NabarroHerring structure. This suggests that the correlation for rupture time should be based on P parameter. Nevertheless, accorng to Filacchioni et al. (199), in this particular case the classical MP is sufficient. Therefore, a correlation based on the arsonmiller parameter has been implemented. Of course, also a stressp correlation can be used, but where possible MP is here preferred because it is usually adopted in the literature. The correlation implemented in the FRoriented version of TRANSURANUS is the following: (16) (17) In Figure 18, the correlation is compared with Filacchioni (199) data. Equivalent stress [MPa] 6 5 K 123 K 2 1 Filacchioni et al., 199 MP/Stress correlation MP = T ( og t R ) Figure 18: MP/stress correlation for AIM1.
35 Sigla identificazione ADPFISS P Irraation creep The irraation creep of the 1515Ti austenitic steels depends on the neutron flux and on the mean neutron energy, along with the stress. The correlation proposed by Többe (1975), reported in Table 14, is already implemented in TRANSURANUS (v1m3j12). Table 14: 1515Ti steels irraation creep correlation. [ ] [ ] [ ] [ ] Reference MPa n cm 2 s 1 MeV h 1 Többe, 1975 Correlation The treatment of the irraation creep in TRANSURANUS The correlation for the irraation creep rate can be expressed in the following general form: (18) where A * is a constant in MPa 1 n 1 cm 2 s h 1 (the unit of measurement is unusual since some conversions have been applied). A similar approach is already adopted in TRANSURANUS for other materials (TRANSURANUS Handbook, 213; Többe, 1975). In these routines, the irraation creep rate is proportional to the flux, and not to the fluence. Obviously, to calculate the irraation creep, the time integration is needed: (19) For this reason, the irraation creep rate is expressed in h 1. The Equation (18) has been implemented following the literature for what concerns the cladng in iquid Metal Reactors (Frost, 1994; Kohno et al., 1999; Toloczko et al., 1996; Toloczko et al., 1998). The relation incated by the literature reads: (2) Where is the irraation creep rate in dpa 1 B is the creep compliance in dpa 1 MPa 1 D is the swelling enhanced coefficient in MPa 1 is the volumetric swelling rate dpa 1 Nevertheless, because of the high uncertainty of the swelling behavior, the approach proposed does not consider the coupling with the swelling  i.e., the second term of the Equation (2). In order to implement this relation in TRANSURANUS, the irraation creep rate has to be converted from dpa 1 in h 1 (i.e., from unit of "dose" to unite of time) accorng to the following relation: (21)
36 Sigla identificazione ADPFISS P Where K is the conversion factor between fluence and "dose" in n cm 2 dpa 1 (a typical value for fast reactor is ) d is the "dose" in dpa t is the time in h (36 is the conversion from hours to seconds) Even if the fluence appears in the previous relation, only the flux is present in the Equation (18) since the irraation creep has to be expressed per unit of time. By means of some substitutions, it is possible to derive the initial equation, Equation (18), where and the irraation creep rate is proportional to the flux and stress. (22)
37 Sigla identificazione ADPFISS P REFERENCES Agosti, F., Botazzoli, P., Di Marcello, V., Pastore, G., uzzi,., 213. Extension of the TRANSURANUS code to the analysis of cladng materials for liquid metal cooled fast reactors: a preliminary approach. Technical Report, CESNEFIN (public version). Aït Abderrahim, H., Baeten, P., De Bruyn, D., Fernandez, R., 212. MYRRHA A multipurpose fast spectrum research reactor. Energ. Convers. Manage. 63, 4 1. Alemberti, A., Frogheri, M., Mansani,., 213. The ead Fast Reactor: Demonstrator (AFRED) and EFR Design. In: Proceengs of the IAEA International Conference on Fast Reactors and Related Fuel Cycles: Safe Technologies and Sustainable Scenarios (FR13), Paris, France, March 34. Banerjee, A., Raju, S., Divakar, R., Mohandas, E., 27. High temperature heat capacity of alloy D9 using drop calorimetry based enthalpy increment measurements. Int. J. Thermophys. 28 (1), Bergmann, H.J., ProjektMaterialdatenhandbuch IV KNKII/3, Revisionsstand 4/88, INTERATOM Bericht/Report B. Bergmann, H.J., Dietz, W., Ehrlich, K., Mühling, G., Schirra, M., 23. Entwicklung des Werkstoffs X1CrNiTiB als Strukturmaterial für Brennelemente. Wissenschaftiche Berichte FZKA 6864, FZK, Karlsruhe. Cacuci, D.G., 211. Chapter 23: eadcooled Fast Reactor (FR) Design: Safety, Neutronics, Thermal Hydraulics, Structural Mechanics, Fuel, Core, and Plant Design. In: Handbook of Nuclear Engineering, Volume 4, ed. Springer, Boston. Cheynet, B., Dubois, J.D., Milesi, M., Données thermodynamiques des éléments chimiques, Techniques de Ingénieur, Matériaux métalliques, No. M153, Form M64. Dubuisson, P., 213. Core structural materials  feedback experience from Phénix. IAEA TECDOC 1689, pp Filacchioni, G., De Angelis, U., Ferrara, D., Pilloni,., 199. Mechanical and structural behaviour of the second double stabilized stainless steels generation. In: Proceengs of the International Conference on Fast Reactor Core and Fuel Structural Behaviour, Inverness, ondon, UK, June 46, pp Friedland, A.J., Coolant Properties, Heat Transfer and Fluid Flow of iquid Metals. In: Fast Reactor Technology: Plant Design, J.G. Yevick (Ed.), Chapter. 2, The M.I.T. Press, Cambridge (MA), USA. Frost, B.R.T., Nuclear Materials, Volume 1B, ed., Materials Science and Technology Series, VCH Verlagsgesellschaft GmbH and VCH Publishers, Inc, Weinheim. García Ferré, F., Ormellese, M., Di Fonzo, F., Beghi, M.G., 213. Advanced Al 2 O 3 coatings for high temperature operation of steels in heavy liquid metals: a preliminary study. Corros. Sci. 77, Gavoille, P., Courcelle, A., Seran, J.., Averty, X., Bourliau, B., Provitina, O., Garat, V., Verwaerde, D., 213. Mechanical Properties of Cladng and Wrapper Materials for the ASTRID FastReactor Project. In: Proceengs of the IAEA International Conference on Fast Reactors and Related Fuel Cycles: Safe Technologies and Sustainable Scenarios (FR13), Paris, France, March 34. Gehr, H.., Datensammlung zur Kernelementauslegung. Interatom  Technischer Bericht 73.3.
38 Sigla identificazione ADPFISS P GIF, 22. A Technology Roadmap for Generation IV Nuclear Energy Systems. Technical Report GIF2. Gurvich,.V., Veyts, I.V., Thermodynamic Properties of Invidual Substances, 4th ed., Vol. 2, Parts 1 and 2, Hemisphere Pub. Corp., New York. Hübner, R., 2. Das Bestrahlungverhalten des austenitischen Stahls DIN 1.497, FZK, Karlsruhe. Hultgren, R., Desai, P.D., Hawkins, D. T., Gleiser, M., Kelley, K.K., Selected Values of the Thermodynamic Properties of Binary Alloys. ASM, Metals Park, Ohio, USA. (accessed ). Iida, T., Morita, Z., Takeuchi, S., Viscosity Measurements of Pure iquid Metals by the Capillary Method. J. Japan Inst. Metals 39, Kirshenbaum, A.D., Cahill, J.A., Grosse, A.V., The density of liquid lead from the melting. J. Inorg. Nucl. Chem. 22, Kohno, Y., Kohyama, A., Hirose T., Hamilton, M.., Narui, M., Mechanical property changes of low activation ferritic/martensitic steels after neutron irraation. J. Nucl. Mater , Kutateladze, S.S., Borishansky, V.M., Novikov, I.I., Fedyaskii, O.S., iquidmetal Heat Transfer Mea. At. Energ., Suppl. 2. (Transl. Cons. Bur. Inc., New York, 1959). Kyrillov, P.I., Deniskina, N.B., 2. Thermophysical Properties of iquid Metal Coolants. Tables and Correlations, Review FEI291, IPPE, Obninsk. ombar, C., 26. Impianti nucleari, Cusl, Milano. ucas,.d., 1984, Données physicochimiques des principaux métaux et métalloïdes. Techniques de l Ingénieur, Matériaux métalliques, N M153, Form M65a. yon, R.N. (Ed.), iquid Metals Handbook, 2nd Ed., Report NAVEXOS P733, Atomic Energy Commission and Dept. of the Navy, Washington, USA (rev. 1954). Nikolopoulos, P., Schulz, B., Density, thermal expansion of stainless steel and interfacial properties of UO 2 stainless steel above 169 K. J. Nucl. Mater. 82, OECDNEA, 27. Handbook on eadbismuth Eutectic Alloy and ead properties, Materials Compatibility, Thermalhydraulics and Technologies. Rudtsch, S., Ebert, H.P., Hemberger, F., Barth, G., Brandt, R., Groß, U., Hohenauer, W., Jaenicke Roessler, K., Kaschnitz, E., Pfaff, E., Pößnecker, W., Pottlacher, G., Rhode, M., Wilthan, B., 25. Intercomparison of thermophysical property measurement on an austenitic stainless steel. Int. J. Thermophys. 26 (3), Ruppersberg, H., Speicher, W., Density and Compressibility of iquid ipb Alloys. Z. Naturforsch. 31 a, Schumann, U., 197. MAPIB, A program system for provision of material property data to computer programs. KFK Smithells Metals Reference Book (8th etion), 24. Gale W.F., Totemeier T.C. (Eds.), Elsevier, Amsterdam. Többe H., Das Brennstabrechenprogramm IAMBUS zur Auslegung von Schellbrüter Brenn  stäben, Technischer Bericht, ITB
39 Sigla identificazione ADPFISS P Toloczko, M.B., Garner, F.A., Irraation Creep and Void Swelling of two MR Heats of HT9 at 4 C and 165 dpa. J. Nucl. Mater , Toloczko, M.B., Garner, F.A., Eiholzer, C.R., Irraation Creep of Various Ferritic Alloys Irraated at 4 C in the PFR and FFTF Reactors. J. Nucl. Mater , TRANSURANUS Handbook, 213. European Commission, JRC, Institute for Transuranium Elements, Karlsruhe. Ushakov, P.A., Zhukov, A.V., Matyukhin, N.M., Heat transfer to liquid metals in regular arrays of fuel elements. Translated from Teplofizika Vysokikh Temperatur 15 (5). Waltar A.E., Todd D.R., Tsvetkov, P.V. (Eds), 211. Fast Spectrum Reactors, Springer, New York. Weisenburger, A, Heinzel, A., Muller, G., Muscher, H., Rousanov, A., 28. T91 cladng tubes with and without mofied FeCrAlY coatings exposed in BE at fferent flow, stress and temperature contions. J. Nucl. Mater. 376,
40 Sigla identificazione ADPFISS P Conclusion and future work The present work has been decated to the extension of the TRANSURANUS code for analyzing the fuel pin behavior of innovative FRs, with reference to the materials adopted in the AFRED design. The material properties of lead as well as of 1515Ti austenitic cladng steels have been implemented in the FRoriented version. The main outcomes of this report may be summarized as follows: The properties of lead have been updated in the TRANSURANUS code. The OECDNEA Handbook has been used as summarized and reasoned reference. In particular, the correlations concerning specific heat capacity, dynamic viscosity, density, heat transfer, boiling temperature, thermal conductivity, enthalpy, boiling pressure, heat of evaporation and corrosion have been updated. A critical review of the main properties of 1515Ti steel has been performed, with the description of the outofpile correlations implemented in the TRANSURANUS code. The properties of the austenitic steels are compared with other literature data in order to assess their vality. Beside this purpose, the comparison has been useful to understand the critical properties which are strongly dependent on the alloying elements and to underline the fferent behavior of the various steels of the 1515Ti family (AIM1, 1.497, D9). In this sense, yield strength, ultimate tensile strength, rupture strain, swelling and thermal creep are features that strongly depend on the composition. The Banerjee correlation for the heat capacity of the 1515Ti steel has been implemented in the code. New correlations for the swelling, the thermal creep strain and the Cumulative Damage Function (CDF, with the introduction of the P parameter) of 1515Ti cladng steels have been implemented in the FRoriented version. This crucial aspect was totally absent in TRANSURANUS before this work. In particular, specific correlations for the 1.497m and the AIM1 steels have been proposed. As natural continuation of this work, we envisage in the future to adopt the FRoriented version for analyzing the fuel pin integral behavior of the AFRED reactor. To this purpose, the capabilities of the TRANSURANUS integral performance code will be exploited to evaluate (on the basis of power history simulations) the synergy of the phenomena occurring throughout the fuel pin life in reactor and their impact on the fuel pin design improvement. In particular, the following results are expected to be suitable for giving important feedbacks to the reactor designers during the conceptual design of AFRED reactor (see also Figure 1, in Introduction): critical analysis of the fuel pin behavior in reactor, along with a sensitivity analysis on the models affected by more uncertainty so as to identify a worst case scenario for the fuel pin performance; careful evaluation of the PCMI dynamics, both in normal operation and accident contions, due to the closing process of the fuel pin gap;
41 Sigla identificazione ADPFISS P optimization of the fuel pin design and performance, in order to achieve enlarged safety margins; identification of the most adequate FA geometrical configuration from the thermomechanical point of view; identification of the main issues on which the R&D activities and efforts should be focused in the near future as far as the behavior of the materials (lead, AIM1 cladng steel, coating, MOX fuel) is concerned. All these future activities are expected to give useful incations for the design of the AFRED reactor and, more in general, for improving the intrinsic safety features of innovative lead cooled FBRs.
42 Sigla identificazione ADPFISS P Part2 Modeling and analysis of nuclear fuel pin behavior for innovative lead cooled FBR: MOX conductivity models
43 Sigla identificazione ADPFISS P CONTENTS 1 INTRODUCTION Objective of the activity Thermal conductivity of ceramic fuel Effect of temperature Effect of stoichiometry Effect of burn up Effect of fuel porosity Effect of Plutonium content TRANSURANUS THERMA CONDUCTIVITY MODES Correlation 31Van Uffelen and Schubert Correlation 32Carbajo Correlation 33anning and Beyer Correlation 34, Wiesenack Comparison among TRANSURANUS models ANAYSIS OF MOX CONDUCTIVITY MODES FROM OPEN ITERATURE D.G Martin review FTHCON subscodematpro The COMETHE formulation Baron Hervè Model COMPARISON BETWEEN THE STUDIED MODES REFERENCES... 75
44 Sigla identificazione ADPFISS P Introduction 1.1 Objective of the activity Among the parameters that governs the myriad of processes that occurs during irraation of fuels rods, the fuel temperature, is by far the most important one (i.e. it dominates the FGR and swelling mechanisms) [1]. The correct prection of the fuel temperature profile is therefore the basis for the simulation of integral fuel rods by means of fuel performance codes. The present report aims to assess the correlations implemented in TRANSURANUS code to simulate conductivity of MOX fuels comparing them with correlations available from open literature. 1.2 Thermal conductivity of ceramic fuel Thermal conductivity is a property representing the ability of a solid material to transfer heat. There are three phenomena considered when modelling thermal conductivity. attice vibrations, raation heat transfer and electronic conductivity [2]. attice vibration thermal conductivity (k latt ) is modelled by assuming the solid to be an ideal gas consisting of phonons. Phonons are quasi particles representing the wave nature of the vibrating solid in the lattice. They tend to collide with each other and with defects in the crystal with a certain mean free path. They transport their energy as they translate in the meum from the hot side to the cold one. Thermal conductivity depends on the amount of energy a phonon can carry and the mean free path of the phonon [3]. Phonon s mean free path should be inversely proportional to the temperature. Due to the presence of point defects in the crystal solid that acts as a barrier to phonon s mobility, the mean free path cannot keep monotonically increasing as the temperatures gets lower [3]. This requires that the mean free path is inversely proportional to temperature plus an extra constant term representing phonon scattering with defects. Being proportional to the mean free path of the phonon, k latt would be written as: Where A, and B are constants, and T is the temperature in (K). Eq.1 Heat is conducted as well with raation on the form of electromagnetic waves. Energy is transported due to the movement of charged particles (protons and electrons) which emit some of their energy on the form of electromagnetic raation [3][4]. Raation term of thermal conductivity (K rad ) is written on the form of a constant times the cube of temperature: Eq.2 At temperatures high enough, energy is sufficient to generate an amount of electronhole pairs that contribute to thermal conductivity (K el ) [3]. Where: ( ) [ ( )] Eq.3 = electronic contribution to thermal conductivity.
45 Sigla identificazione ADPFISS P = Boltzmann constant, 1.38x1 23 (J/K) = electron charge, 1.6x119 (Coul) = electron/hole contribution to electrical conductivity ( ) ( ) = energy gap between conduction and valence bands (J) Where the first term on the RHS is the conductivity effect of holes and electrons separately. The second term represents the ambipolar effect, which is the release of the kinetic energy of both the electron and hole when they recombine together plus the release of their generation energy at areas of lower temperature leang to the transfer of heat electronically. This equation can be simplified using some experimental data and assumptions to be written on the form: [2] Eq.4 Where D,E and n are constants, it should be noted that n ffers from one model to another. These physical principles of heat conduction and their equation forms are generally taken into account in the models even if they can be implemented in fferent ways. Most of these models account only for the first two thermal conductivity principles. 1.3 Effect of temperature Thermal conductivity of UOx and MOX is a property that depends on temperature. It has been noted experimentally that the thermal conductivity decreases with temperature until a plateau is reached in the range between 15 to 2 C. This decrease is due to the lattice vibration conductivity, which is inversely proportional to the temperature. At temperatures above the plateau range, the thermal conductivity begins to rise again. This is attributed to either of the two other components of the thermal conductivity. Raation heat conduction takes place above the plateau temperature even though it is not that much significant. Electronic term of the thermal conductivity is the second term that is responsible for the increase of thermal conductivity. The lattice vibration mechanism is included in all the models. As usual, it takes into consideration other factors that affect the heat conductivity other than temperature (e.g. burn up rate, deviation from stoichiometry, etc). Some models, take the raation conduction term into consideration to explain the increase of thermal conductivity at higher temperatures, while others relate that increase to the electronic conduction term. 1.4 Effect of stoichiometry The theoretical oxygen to metal ratio (O/M) between Uranium or Plutonium oxide (UPu)O 2 is two. Deviation from this value are generally adopted by design and are also induced in the nuclear fuel aseffect of irraation. The deviation can lead to hyper (>2) or hypo (<2) stoichiometric state of the fuel [6].
46 Sigla identificazione ADPFISS P The effect of deviation from stoichiometric is generally modeled by assuming that this deviation causes more defects in the lattice. This perturbation is included in the constant A in Eq.1 which represents the phonondefect interaction in the lattice and determined originally for stoichiometric fuel contions. The mofication of due to deviation from stoichiometry can be written as Eq.5 Where is the constant A for stoichiometric fuel and C is a constant multiplied by which is the deviation form stoichiometry (O/M2)). 1.5 Effect of burn up The irraation process that takes place in a nuclear reactor leads to various changes in the properties of the fuel rod. Defects in the lattice, porosity increase, deviation from stoichiometry and fuel cracking with irraation leads to degradation of the thermal conductivity. This effect is important in fast reactors since burn up can reach to more than 1% of the original weight content of the uranium and plutonium [6]. Solid fission products have fferent effects on thermal conductivity. In general, those that are ssolved tend to decrease the thermal conductivity, while those that are precipitated tends to increase it. The integral effect is however a degradation of conductivity with increasing burnups. 1.6 Effect of fuel porosity The presence of voids in the solid fuel pin leads to degradation of its thermal conductivity. A poreless fuel is required to obtain the maximum thermal conductivity. On the other side, the presence of pores in the fuel pin is important to accommodate the release of fission gases that are formed during irraation. Theses fission gases can cause internal pressure of the fuel pin to increase leang to deformation and swelling of the fuel. This effect is more important for fast reactors than thermal reactors because the higher power density leads to more generation of fission gases [6]. The porosity (P) is defined as the volume of the pores inside the fuel vided by the total volume of the fuel this can be written as: Eq.6 Where is the actual density of the fuel, and is the theoretical density of the fuel s material without pores. The effect of porosity on thermal conductivity is considered by using a correction factor of the thermal conductivity. This factor has many formulations but the most used are the mofied oeb formula: or the MaxwellEucken formula: Eq.7 Eq.8
47 Sigla identificazione ADPFISS P Where is the thermal conductivity of the poreless fuel. α and β are constants. Theoretically, the values of α is 1 and β is.5. Experimentally, the noticed values of these factors are higher than what the theory prects. This is due to the fact that the pores are not randomly stributed in the lattice which is theoretical assumption [7]. The wide range of values used for the constants α and β shows that they are in fact variables that depend on the pore shape. The values assigned to them represents an average of the porosity effect. 1.7 Effect of Plutonium content The effect of Plutonium on the constants A and B in the lattice vibration thermal conductivity term has been carefully stued. Evidence does not show any systematic trend for the variation of the constant A, while it shows a systematic increase of the constant B. Overall the effect of increasing Plutonium s content in the fuel is a decrease of the thermal conductivity of MOX fuel [3]. This decrease reaches up to 15% for a plutonium content of around 25 wt.%.
48 Sigla identificazione ADPFISS P TRANSURANUS thermal conductivity models This section provides an assessment and a comparison of the correlations adopted in TRANSURANUS to simulate MOX fuel conductivity. 2.1 Correlation 31Van Uffelen and Schubert This correlation is based on the data obtained experimentally by Duriez et.al where the laser flash technique was used to measure the thermal ffusivity of MOX fuel. The Pu content of the fuel was between 315%.wt, O/M ratio between and in the temperature range between 723 K [9]. The the thermal conductivity was modeled by using values of the heat capacity calculated from Kopp s law [8]. The ambipolar electronic thermal conductivity term is based on the work of Ronchi et.al in which they measured the thermal ffusivity and the heat capacity of UO 2 for a temperature range between 5 and 19 using an advanced laserflash technique that gave better results than conventional laser flash methods at high temperatures [9]. The correlation gives the thermal conductivity of MOX as a function of temperature and burnup: Where a=.38 a1 =5.498x13 b=2.515 x14 b1= x16 c= 4.715x x1 9 d=16361 Eq.9 T is in K and = min(1923,t), bu is the local burn up in The porosity effect can be taken into account using the following correction formula Eq.1 This correlation has been assessed assuming fferent contions. Due to the lattice vibration term, the correlation prects a decrease of thermal conductivity for fuel with temperature until it reaches a minimum around 2 K and then begins to rise again due to the electronic heat conduction as shown in Fig.1. This figure assumes a fuel of 95% theoretical density and includes fferent level burnups. The effect of burn up on the thermal conductivity is more important at lower temperature. As can be seen in Fig.1, at 8 K the thermal conductivity decreased by 6% of its original value for unirraated fuel when the burn up reached 1. For 2 K, the thermal conductivity for the same range of burn up decreases only by 1%. It is noticed as well that the higher burnup, the lower the rate of change of thermal conductivity with temperature. Also as the burnup increases, the lower the temperature for which the thermal conductivity reaches its minimum before it increases again. At burn up of 1, the thermal conductivity is slightly changing with
49 Sigla identificazione ADPFISS P temperature until the temperature is above 15 K where the effect of the ambipolar term of thermal conductivity starts to rise. This behavior is explained by the increase of the defects in the solid due to irraation. As consequence of this the phonondefect interaction in the fuel dominates with respect to hte temperature dependent phononphonon interaction term. Fig.1  Thermal conductivity as a function of temperature for fferent burn ups, correlation 31. The effect of porosity is analyzed in Fig.2 (under the assumption of unirraated fuel). The correlation prects a decrease of thermal conductivity with porosity. This decrease is linear and the rate of decrease is constant over the whole range of temperatures. It is between 2 to 25% in thermal conductivity when the porosity increase from to 1%. In Fig.3, The contributions of the lattice vibration and the ambipolar thermal conductivity are plotted accorng Van Uffeleln & Schubert correlation. This is done for this correlation only to illustrate what was explained before in theory related to the dominating contribution of lattice vibration term at low temperatures. At low temperatures the main contribution to the total thermal conductivity is the one related the lattice vibration. As the temperature increases, this term keeps decreasing combined with the increase of the electronic term. When the rate of increase of electronic thermal conductivity dominates the rate of decrease due to lattice vibration the thermal conductivity begin to rise again. This domination takes place in the temperature range between (162 K).
50 Sigla identificazione ADPFISS P Fig.2  Effect of fuel porosity on thermal conductivity, correlation 31. Fig.3  Comparison between the lattice and the ambipolar contribution to the total thermal conductivity. 2.2 Correlation 32Carbajo This correlation is based on the work of Carbajo et.al. that take basis for best value estimation of data available from open literature available recommendations given in other works. The physically based correlation by ucuta et.al was recommended. It gives the thermal conductivity as a function of temperature, burnup, deviation from stoichiometry along with a porosity correction. The
51 Sigla identificazione ADPFISS P correlation takes the fuel irraation into account as well as the effect of ssolved and precipitated solid fission fragments as a separate function from the unirraated fully dense fuel elementerrore. 'origine riferimento non è stata trovata.. The thermal conductivity for a 1%TD MOX fuel is given by ( ) Eq.11 Where =.35, =2.85, =.286, b1= .715, c= 64 and d=16.35 X is the deviation from stoichiometry, = and T is the temperature in [K] The factor FD represnts the negative effect of ssolved fission fragments on the thermal conductivity and is defined as: [ ] Eq.12 For > and Eq.13 where ( ) Eq.14 is the burnup in at.% The factor FP represents the increase in thermal conductivity due to the precipitaed solid fission products: [ ( )] Eq.15. The factor FR accounts for raation effects. It is important below 9 K and reaches near unity rapidly above 9K and does not play a significant role above that temperautre. ( ) The porosity effect is modelled using the MaxwellEuckman correction formula Eq.16 Eq.17
52 Sigla identificazione ADPFISS P The correlation prects a decrease of thermal conductivity with temperature due to lattice vibration until it reaches a minimum around 2 K. Then, it begins to rise again due to the electronic heat conduction as shown in Fig.4 for a 95%TD fuel at fferent burn ups. The same is true for fferent values of fuel porosity. It can be noticed as well the decrease of thermal conductivity with burn up. The effect of burn up on the thermal conductivity is more important at lower temperature. As can be seen from Fig.4, at 8 K, the thermal conductivity decreased by 4% of its original value for unirraated fuel when the burn up reached 1 at.%. For 2 K, the thermal conductivity for the same range of burn up decreases by 15%. Fig.4  Thermal conductivity as a function of temperature for fferent burn ups, correlation 32. The effect of porosity is analyzed infig.5 (for unirraated MOX). The decrease of conductivity with increased porosity is linear and the rate of decrease is constant over the whole range of temperatures. It is between 2 to 25 when the porosity increase from to 1%. The effect of O/M is reported in Fig.6 and Fig.7 (for unirraated MOX). The correlation is physical for the hypostoichiometric section while, for the deviation in the rection of hyperstoichiometry, the correlation does not give physical results since it prects the increase of thermal conductivity, Fig.6 (that is in contraction with the theoretical and experimental finng that hilight a maximum of condutivity for O/M = 2 and lower values for all the other ratios). Due to this reason, further analyses are conducted only up to O/M = 2, Fig.7. It sholud be pointed out that the code recommends the use of these correlations only for O/M up to 2. It can be noticed that the lower the temperature, the higher the degradation of thermal conductivity with deviation from stoichiometry. For 8 K the thermal conductivity decreases by 3% for a deviation from stoichiometry of.5. At 2 K for the same range of deviations, the decrease of thermal conductivity is around 8% and decreases more as the temperature goes higher.
53 Sigla identificazione ADPFISS P Fig.5  Effect of fuel porosity on thermal conductivity, correlation 32. Fig.6  effect of deviation from stoichiometry on thermal conductivity at fferent values of temperature, correlation 32.
54 Sigla identificazione ADPFISS P Fig.7  Thermal conductivity as a function of temperature for fferent burn ups, correlation Correlation 33anning and Beyer This correlation gives the thermal conductivity for 95%TD MOX accorng to anning and Beyer. The correlation is based on the work of Duriez et al. [8] It gives the thermal conductivity as a function of temperature, burn up and deviation from stoichiometry included in the lattice vibration term and another term for ambipolar thermal conductivity that is a function of temperature only. The thermal conductivity for MOX 95%TD is given by: Eq.18 Where: X is the deviation from stoichiometry and T is in K and the burn up is in.
55 Sigla identificazione ADPFISS P A porosity correction term accorng to ucuta applies to obtain the thermal conductivity at fferent real densities. The porosity correction is on the form of MaxwellEuckman formula: ( ) Eq.19 The correlation prects decrease of thermal conductivity with temperature until it reaches a minimum between 185 and 19 K then begins to rise again due to the electronic heat conduction as shown in Fig.8 for a 95%TD of the fuel at fferent burnups. The same is true for fferent values of fuel porosity. It can be noticed as well that the decrease of thermal conductivity with burnup which is consistent with the other MOX correlation used in TRANSURANUS and the theoretical expectations. Again, the effect of burnup on the thermal conductivity is more important at lower temperature as can be seen from Fig.8 being the degradation of conductivity in the order of 4% at 8K (in the range 1MWd/kgHM). At 2 K, the thermal conductivity for the same range of burnup decreases by 18%. Porosity effect is given in Fig.9. The decrease is linear and the rate of decrease is constant over the whole range of temperatures (it is about 15% when the porosity increase from to 1%). Deviation from stoichiometry is accounted in Fig.1 and Fig.11. The more hypostoichiometric the fuel, the higher the decrease of the thermal conductivity. For a change of O/M from 2 to 1.95, the decrease in thermal conductivity can reach upto 3% at 8 K. This effect gets lower as the temperature goes high. At 2 K and the reduction in thermal conductivity on the same range of change of O/M ratio is about 8%, as noticed in Fig.1. It is known that the thermal conductivity decreases with temperature to a minimum then increases again. It can be notice from Fig.1. that the more hypostoichiometric the fuel is the lower the temperature for which the thermal conductivity reaches that minimum. As in the previous case, the correlation is non physical for hyperstoichiometry since it prects the increase of thermal conductivity with hyperstoichiometry which contracts the experimental finngs. It sholud be pointed out that the code recommends the use of these correlations only for O/M up to 2. The lower is the temperature, the higher is the degradation of thermal conductivity with the hypostoichiometry, Fig.11. For 8 K the thermal conductivity decreases by 3% for a deviation from stoichiometry of.5. At 2 K for the same range of deviations the decrease of thermal conductivity is around 8% and decreases more as the temperature goes higher.
56 Sigla identificazione ADPFISS P Fig.8  Thermal conductivity as a function of temperature for fferent burn ups, correlation 33. Fig.9  Effect of fuel porosity on thermal conductivity, correlation 33.
57 Sigla identificazione ADPFISS P Fig.1  Effect of deviation from stoichiometry on thermal conductivity at fferent values of temperature, correlation 33. Fig.11  Thermal conductivity as a function of temperature for fferent burn ups, correlation 33.
58 Sigla identificazione ADPFISS P Correlation 34, Wiesenack. Correlation 34 is the original Wiesenack s correlation that is developed for UO 2 fuel. In order to apply it for MOX, the correlation is multiplied by a correction factor of.92. The original correlation gives the thermal conductivity of MOX as a function of temperature and burnup on the form: { } { } Eq.2 Where:.188 And is the temperature in [ C] and bu is the burn up in There is no specific equation for porosity correction given for this model so the original MATPRO 11 porosity correction is used: Where P is the porosity and Eq.21 The correlation prects a decrease of thermal conductivity with temperature until it reaches a minimum between 17 and 19 K. For unirraated fuel, the minimum of thermal conductivity is reached at 19 as shown in Fig.12. The correlation incates that as the burn up of the fuel increases, that minimum in thermal conductivity is reached at a lower temperature. The minimum in thermal conductivity at burn up of 1 is reached at a temperature range between 15 to 16. It can be noticed as well that the higher the burn up the flatter the curve of thermal conductivity at lower temperature before it increases rapidly again at higher temperature. This gives an incation that the phononphonon lattice vibration term is not effective and that the constant term related to the phonondefect interaction is the dominant one leang to almost constant thermal conductivities at the range in which the thermal conductivity is more dependent on lattice vibration rather than electronic conductivity. The thermal conductivity begins to rise again in the range of temperature in which the ambipolar conductivity is dominant. The effect of burn up on the thermal conductivity is higher at lower temperature as shown in Fig.12 At 8 K the thermal conductivity decreased by 55% of its original value for unirraated fuel when the burn up reached 1 2 K, the thermal conductivity for the same range of burnup decreases by 25%. The burn up at temperatures higher than 2K seems to have a constant effect. The amount of thermal conductivity decrease is the same regardless of the initial level of thermal conductivity. The curves appear to be parallel to each others as can be seen in Fig.12. The correlation prects (Fig.13) a decrease of thermal conductivity with porosity. This decrease in thermal conductivity is about 22% at low temperature (8 K) when the porosity increases from %. For
59 Sigla identificazione ADPFISS P to 1%. On the same range of variation of porosity, as the temperature increases to 19 the decrease of thermal conductivity with porosity decreases to 11%. Fig.12  Thermal conductivity as a function of temperature for fferent burn ups, correlation 34. Fig.13  Effect of fuel porosity on thermal conductivity, correlation 34.
60 Sigla identificazione ADPFISS P Comparison among TRANSURANUS models The correlations implemented in TRANUSURANUS code described above are compared in Fig. 14 and Fig.15. The thermal conductivity change with temperature for unirraated 95% TD MOX fuel is given in Fig. 14. The two correlations that has the effect of deviation from stoichiometry as variables are ploted for two limits of 2 (stoichiometric contion) and 1.96 to see the range of changes due to deviation from stoichiometry. One can notice from Fig. 14 that the highest prected thermal conductivity for the whole temperature range is that for the Weisenak correlation (correlation 34) that is originally developed for UO 2 fuel with a correction factor to make it applicable for MOX. anning and beyer s correlation for stoichiometric contion gives values that are comparable to that of the mofied Weisenak correlation. The more hypostyoichiometric the fuel becomes, the higher deviation between the two correlations exists. Correlation 31 accorng to Van Ufflen and Schubert is identical to that of anning and Beyer (correlation 33) at lower temperature. As the ambipolar thermal conductivity term begins to dominate, Correlation 33 deviates to a lower values from that of Correlation 31 which is similar with the thermal conductivity accorng to Carbajo (correlation 32). Correlation 32 gives a lower value of thermal conductivity from the other correlations at stoichiometric contions. At temperatures below 1 K then, it becomes similar with them in the intermeate temperature range then follow the same path as correlation 31 and deviates again to lower values than that of correlation 32 and 34. For the same theoretical density and with burnup up to 1, the rate of degradation of thermal conductivity accorng to correlation 34 is the highest for most of the temperature range of interest leang to higher decrease of thermal conductivity. The thermal conductivity by that correlation is now comparable to those for the hypostoichiometric (O/M =1.96) correlations. Stoichiometric correlations 32 and 33 have the lowest rate of decrease of thermal conductivity with burn up and at the level of 1 they prect the highest thermal conductivities among all the correlations. Fig.14  Thermal conductivities from TRANSURANUS correlations.
61 Sigla identificazione ADPFISS P Fig.15  Thermal conductivities from TRANSURANUS correlations.
62 Sigla identificazione ADPFISS P Analysis of MOX conductivity models from open literature In this section, several open literature correlations are described along with the variables that are considered. The form of the equation for each model along with comments on the results obtained from these correlations are included. 3.1 D.G Martin review 1982 In this work Martin d a reappraisal of four thermal conductivity correlations (Washington, Anscough, Killeen and Brandt) and chose one of them to do some ammendments to it instead of producing a new independent correlation. The correlation chosen was that based on Washington s review in Even though the correlation by Killeen was the most correlation based on theory for stoichiometric fuel, There were no theoretical knowledge sufficient enough to apply it with certainity on nonstoichiometric fuel. The two correlations (Fig.16) are close to each other at low and high temperature range, and even in the intermeate one, the deviation of Washington s correlation from that of Killeen should not cause great errors. [7] The data available were reappraised and the few new data that appeared since the work of Washington were added to the review. The correlation seemed to be giving satisfactory results for UO 2 and MOX as a function of temperature and O/M ratio. The amended correlation can be written for hypostoichiometric MOX as: Eq.22 The original correlations were tailored for UO2 and were projected to MOX by assuming a correction factor of.95.the new correlation neglected the effect of irraation in the temperature range of (528 C) and the effect of plutonium content. It took the O/M ratio into account in the lattice vibration term. The porosity correction was based on a mofied oeb forumula for porosity level between (<P<.1 ) and based on MaxwellEuckman formula in the range of (.1<P<.2). The effect of porosity is a linear decrease of thermal conductivity as the porosity increases. This decrease reaches to 42% for a porosity increase from to 2% as shown in Fig.17 The effect of deviation from stoichiometry is a degradation of the thermal conductivity. This effect is prected from this correlation as shown in fig. to be from 42% at temperature of 8 K and decreases with temperature to a value of 18% at 2K for a stoichiometry change between (2 and 1.95). The effect of stoichiometry keeps decreasing with temperature but it can be considered important on the whole range of normal operation of a fast breeder reactor fueled with MOX.
63 Sigla identificazione ADPFISS P Fig.16  Thermal conductivity accorng to the four reappraised models by Martin. Fig.17  Effect of fuel porosity on thermal conductivity, Martin.
64 Sigla identificazione ADPFISS P Fig.18  Thermal conductivity as a function of temperature for fferent stoichiometries, Martin. 3.2 FTHCON subscodematpro The correlation used by the FTHCON subroutine determines the thermal conductivity of uncracked UO 2 and MOX fuels as a function of temperature, O/M ratio and plutonium content of a solid fuel. It uses a porosity correction based on the MaxwellEucken relation. The burnup is used only to calculate the melting temperature of the fuel. Interpolation is used to remedy the scontinuity of the slope in the temperature range between ( K). The correlation can be written as follows for Solid fuel: [ ] [ ] [ ] { [ ] } Eq.23 Where: K = Thermal conductivity (W/m.K) D = fractional theoretical density = Phonon contribution to the specific heat at constant vlume (J/kg.K). MATPRO correlation for specific heat is used to calculate this factor = inear strain caused by thermal expansion for temperatures above 3 K. MATPRO correlation for linear strain is used to calculate this factor for uranium and plutonium then the value is weighted accorng to the percentage of Plutonium in the fuel. A = a factor represents the point defect contribution to the phonon s mfp. = X where X is the absolute value of the deviation from stoichiometry
65 Sigla identificazione ADPFISS P B= a factor representing the phononphonon scattering contribution to the thermal conductivity. =.6867( PU) where PU is the weight fraction of the plutonium content of the fuel. T = Fuel temperature in (K) = Fuel temperature if <1364. For temperature higher than 1834 then { } For intermeate range (1364<T<1834), linear interpolation is used to obtain the value of = Fuel temperature if T<18 25 if T> 23 Between (18<T<23)inear interpolation is used to obtain the value of The expected standard error for this correlation is as follows Even though the deviation from stoichiometry is included in the model as a parameter determining thermal conductivity, the model does not show any sensible change of thermal conductivity with deviation from stoichiometry. Fig.19 shows the magnitude of fference of thermal conductivity for a deviation from stoichiometry of.5. The maximum change of thermal conductivity at temperature of 5 K is less than 2% and decreases more with temperature to reach less than.3% at 3 K. The model (Fig.2) prects a change of thermal conductivity between (12 to 9)% with the plutonium content ( to 3%.wt) between 5K and 225 K respectively. This shows a rate of decrease of (.4 to.3%) for every 1%.wt increase in Plutonium content. The results shows that the Thermal conductivity of The model is more dependent on Plutonium content than on deviation from stoichiometry. In Fig.21, the thermal conductivity is plotted as a function of temperature for fferent values of plutonium content for stoichiometric fuel at 95%.TD. The figure shows the results that were illustrated in Fig.2 as a function of temperature.
66 Sigla identificazione ADPFISS P Fig.19  Difference between thermal conductivities measured at O/M f 2 and 1.95 plotted as a function of temperature. Fig.2  Thermal conductivity as a function of plutonium content of the fuel.
67 Sigla identificazione ADPFISS P Fig.21 Thermal conductivity as a function of temperature for fferent Plutonium contents. 3.3 The COMETHE formulation1982 This formula is used for UO 2 and MOX fuels. It gives thermal conductivity of 95%TD fuel. A porosity correction is used to give the thermal conductivity at fferent porosities. It was enhanced to take the plutonium weight percentage into account based on the data from Gibby, Van Craey and weilbacher. [11] The formula is written as follows Where T = temperature (K) X = absolute value of deviation from stoichiometry q= Plutonium content = 4.5 = = 162 =.8 C =.6416x112 ( Eq.24 The model prects (Fig.22) a decrease in thermal conductivity at lower temperature of about.5% for every 1%.wt increase in the Plutonium content for stoichiometric fuel. The rate of decrease slightly decreases at 2 K but still in the same range of.5% per 1%.wt increase in Pu content implying a constant effect of plutonium content on the whole temperature range of interest under normal operations. The effect of deviation from stoichiometry (from 2 to 1.95) is illustrated in Fig.23. The decrease of thermal conductivity with hypostoichiometry can reach up to 42% decrease in thermal conductivity at lower temperatures (8 K). This effect decreases with temperature to reach around 18% decrease with stoichiometric decrease from 2 to For the whole range of temperatures of interest the change of thermal conductivity with deviation from stoichiometry is higher than that due to increase of plutonium content of the fuel.
68 Sigla identificazione ADPFISS P Fig.22  Thermal conductivity as a function of temperature for fferent plutonium contents. Fig.23  Thermal conductivity as a function of temperature for fferent O/M ratios.
69 Sigla identificazione ADPFISS P Baron Hervè Model The model is a mofication of the same model that originated in The mofication concerns the high temperature term. It included originally a term relating high temperature conductivity to raation. The mofication substituted this term by another one that considers electronic thermal conductivity instead. This was done based on the work be Delette and Charles. [11] The model takes the temperature, deviation from stoichiometry, plutonium and Gadolinium content as variables. In order to apply this model to MOX fuel, The Gadolinium content should be set to zero. Eq.25 Where: =Boltzmann constant ( J/K) W= (1.41*1.6)*119 J = (m.k/w), =4, =.611 (m.k/w), =11.81(m.K/W) = (m/w), =.8, = (m/w), = (m/w) C= (W.K/m) D= (W.K/m) And, T is temperature in K up to 26 K, x is the absolute value of deviation from stoichiometry, q is the plutonium weight content, and g is the Gadolinium weight content. The model prects the same effect of Plutonium as in the Comethe formulation. In Fig.24 a decrease in thermal conductivity at lower temperature of about.5% for every 1%.wt increase in the Plutonium content for stoichiometric fuel. The rate of decrease slightly decreases at 2 K but still in the same range of.5% per 1%.wt increase in Pu content implying a constant effect of plutonium content on the whole temperature range of interest under normal operations. The effect of deviation from stoichiometry (from 2 to 1.95) is illustrated in Fig.25. Similar to the COMETHE formulation, the decrease of thermal conductivity with hypostoichiometry can reach up to 42% decrease in thermal conductivity at lower temperatures (8 K). This effect decreases with temperature to reach around 18% decrease with O/M ratio decrease from 2 to For the whole range of temperatures of interest, the change of thermal conductivity with deviation from stoichiometry is higher than that due to increase of plutonium content of the fuel. Comparing the COMETHE formulation and BaronHervè model, the values of thermal conductivity at temperatures up to 2K are comparable. Above 2 K, It can be noticed that the thermal conductivity increases on a higher rate for BaronHervè model than for COMETHE formulation.
70 Sigla identificazione ADPFISS P Thermal conductivity of MOX FUE (W/mK) %.wt Pu 1%.wt Pu 2%.wt Pu 3 %.wt Pu 4 %.wt Pu MOX 95%TD, O/M = Temperature (K) Fig.24  Thermal conductivity as a function of temperature for fferent plutonium contents.
71 Sigla identificazione ADPFISS P Fig.25  Thermal conductivity as a function of temperature for fferent O/M ratios.
72 Sigla identificazione ADPFISS P Comparison between the stued models. In Fig.26, All the stued models are plotted together. For the models that include the deviation from stoichiometry as a variable, the correlations are plotted for fresh fuel, for two limits of stoichiometry (2 and 1.96). This is due to the significant effect of deviation from stoichiometry on thermal conductivity. Meanwhile there are models that do not consider this effect, so it was needed to see the prection of both types of models together and how the deviation from stoichiometry leads to higher variability between the models. In Fig.26, The TRANSURANUS models are plotted with solid lines while the open literature correlations are in dashed lines at O/M ratio of 2. The open literature correlations are plotted with dots at O/M=1.96. FOR (O/M=2), It can been seen that MATPRO at 2%.wt Plutonium and Martin s values of thermal conductivity are higher than TRANSURANUS models for all values of temperatures considered. The values of COMETHE formulation for 2%.wt Plutonium is following Wiesenack s correlation upto 16K then becomes slightly higher than it, then becomes lower again at 21K. The COEMTHE formulation gives higher thermal conductivities than the rest of TRANSURANUS correlations for the shown range of temperature, except at 22K when anning and beyer s correlations starts to give higher values of thermal conductivities. Baron and hervè s correlation for 2%.wt Pu gives lower values than TRANSURANUS correlations except Carbajo s correlation upto 11K where it becomes slightly lower but comparable to Carbajo and (Van Uffelen and Schubert) upto 18 K where it starts to give higher values than both of them but still lower than Wiesenack and (anning and Beyer). At 22K, it starts to become higher than anning and beyer but still lower than Weisenack. In Fig.27, The same plot as in Fig.26 is done but the Plutonium content was reduced to 1%.wt. TRANSURANUS correlations do not consider Pu content so they remain the same. The situation is the same for Martin s review. As for MATPRO correlation an expected increase in Thermal conductivity occurs. The rate of increase of thermal conductivity for COMETHE formulation is stronger than for MATPRO. The thermal conductivities prected by COMETHE is now higher than Martin s and almost comparable to MATPRO below 1K. With more decrease of Pu content, COMETHE becomes higher than MATPRO for temperature upto 11 for pure UO 2. For BaronHervè correlation, As the Pu content increase, thermal conductivity increases and follows Martin s at temperature upto 11 K then follows Weisenack s correlation for the rest of the temperature range. In Fig.26 when O/M ratio is reduced to It is obvious at lower temperatures that the open literature correlations, except MATPRO, prect a higher degradation with deviation from stoichiometry than TRANSURANUS correlations that takes O/M ratio into account (Carbajo anning and beyer). At 17 K it can be noticed that Martin review and COMETHE formulation begins to follow Carbajo s correlation. For the whole range of temperature, Baron and hervè s correlation is lower than all the others except below 95 K where it is slightly higher than Martin s review. With O/M and Pu content decreased to 1.96 and 1%.wt Fig.27, the open literature correlations that takes Pu content into account are still lower than Transuranus correlations in general. COMETHE
73 Sigla identificazione ADPFISS P formulation is higher than Carbajo for T<9 K then decreases up to 16 where it becomes higher than Carbajo again but still lower than anning and beyer for the whole range of temperature. Baron and Hervè s correlation becomes higher than Martin s up to 13 K. It decrease again upto 215 K where it increases again. It this section there were no need to plot another figure at higher burnup value since this was done in section 2.5 for TRANSURANUS correlations. The open literature correlations that were stued here do not have burnup as a variable. So the figure is expected to be a plot where TRANSURANUS prected thermal conductivites degrade with burnup for the same porosity and stoichiometry level and the open literature remains in their high level. It is important to note that even if the open literature models do not take burnup as an explicit variable affecting thermal conductivity, it does not mean that the thermal conductivity would not degrade with irraation. It means that with irraation, the fuel structure would change and it would have fferent level of porosity and stoichiometry and that would lead to a degradation of thermal conductivity with burnup. So, in order to compare TRANSURANUS correlations that takes burnup as an explicit variable with the considered open literature correlations at higher burnup, one must compare them with open literature correlations at a fferent level of porosity and stoichiometry corresponng to the new level of burnup which is out of the scope of this study for now. Finally a comparison is made between Martin s review and COMETHE formulation and the physically based correlation of Killeen. This is done for stoichiometric fuel with 2%.wt Pu content. This is justified by what Martin recommendations in his paper [7] that Killeen s equation is more preferred but due to lack of knowledge of how to project this correlation to nonstoichiometric fuel, Washington s recommendation was considered a suitable substitute. It can be noticed from Fig.28 that COMETHE formulation is consistent with Washington s equation at lower temperature range upto 1K where there is a slight deviation between the two upto 13K. Then the COMETHE formulation follows Killeen s model better than the review of Martin. From 23 K both correlations deviates from Killeen s model. COMETHE correlation has larger deviation from Martin s review than Martin s at high temperatures.
74 Sigla identificazione ADPFISS P Fig.26  Thermal conductivity models of TRANSURANUS and open literature models at 2%.wt Pu.
75 Sigla identificazione ADPFISS P Fig.27  Thermal conductivity models of TRANSURANUS and open literature models at 1%.wt Pu.
Main Process for the logical control of the HELENA loop. I. Di Piazza, M. Tarantino, P. Gaggini. Report RdS/2013/052
Inserire logo o denominazione del cobeneficiario Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DEO SVIUPPO ECONOMICO Main Process for the logical control
More informationReport sull'accoppiamento di Codici CFD e Codici di Sistema. F. Moretti, M. Lanfredini, L. Mengalli, F. D'Auria. Report RdS/PAR2013/043
Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DELLO SVILUPPO ECONOMICO Report sull'accoppiamento di Codici CFD e Codici di Sistema F. Moretti, M. Lanfredini,
More informationStudi Preliminari di Tecniche di Monitoraggio del Nocciolo di ALFRED
Inserire logo o denominazione del cobeneficiario Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DEO SVIUPPO ECONOMICO Stu Preliminari Tecniche Monitoraggio
More informationFlameless Technology for Particulate Emissions Suppression
Flameless Technology for Particulate Emissions Suppression M. Malavasi, C. Allouis, A. D'Anna Report RSE/2009/108 Ente per le Nuove tecnologie, l Energia e l Ambiente RICERCA SISTEMA ELETTRICO Flameless
More informationNumerical Analysis Flow Blockage Phenomena in the ALFRED FA: Preliminary Study on Neutronic Feedback. Ivan Di Piazza, Patrizio Console Camprini
Inserire logo o denominazione del cobeneficiario Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DEO SVIUPPO ECONOMICO Numerical Analysis Flow Blockage
More informationEUROLAB 25 years. The role of metrology and testing to characterize materials and products. EUROLAB 25th Anniversary Seminar
EUROLAB 25 years The role of metrology and testing to characterize materials and products April 9, 2015, Odense Danmark 1 Origin of Conformity Assessment The New Approach for the European Economic Community
More informationTHE COMPARISON OF THE PERFORMANCE FOR THE ALLOY FUEL AND THE INTERMETALLIC DISPERSION FUEL BY THE MACSISH AND THE DIMAC
THE COMPARISON OF THE PERFORMANCE FOR THE ALLOY FUEL AND THE INTERMETALLIC DISPERSION FUEL BY THE MACSISH AND THE DIMAC ByoungOon Lee, BongS. Lee and WonS. Park Korea Atomic Energy Research Institute
More informationDer Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen
Der Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen Tagung des Arbeitskreises Thermophysik, 4. 5.3.2010 Karlsruhe, Deutschland E. Kaschnitz Österreichisches GießereiInstitut
More informationGeneration IV Fast Reactors. Dr Richard Stainsby AMEC Richard.Stainsby@amec.com
Generation IV Fast Reactors Dr Richard Stainsby AMEC Richard.Stainsby@amec.com Contents The Generation IV international research programme on advanced reactors The case for fast reactors The technology:
More informationRICERCA DI SISTEMA ELETTRICO
Agenzia Nazionale per le Nuove Tecnologie, l Energia e lo Sviluppo Economico Sostenibile RICERCA DI SISTEMA EETTRICO Analysis of the impact of the heavy reflector of a typical large size GEN III+ reactor
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationGENERAL PROPERTIES //////////////////////////////////////////////////////
ALLOY 625 DATA SHEET //// Alloy 625 (UNS designation N06625) is a nickelchromiummolybdenum alloy possessing excellent resistance to oxidation and corrosion over a broad range of corrosive conditions,
More informationDatabase of thermophysical properties of liquid metal coolants for GENIV
SCIENTIFIC REPORT SCK CENBLG1069 Database of thermophysical properties of liquid metal coolants for GENIV Sodium, lead, leadbismuth eutectic (and bismuth) Vitaly Sobolev November 2010 (rev. Dec. 2011)
More informationRisk Analysis of Nuclear Power Plants against External Events. L. Burgazzi, N. Davidovich, P. Meloni, R. Lo Frano. Report RdS/PAR2013/089
Inserire logo o denominazione del cobeneficiario Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DEO SVIUPPO ECONOMICO Risk Analysis of Nuclear Power
More informationRDCH 702: Lecture 10 Radiochemistry in reactors
RDCH 702: Lecture 10 Radiochemistry in reactors Readings: Radiochemistry in Light Water Reactors, Chapter 3 (on readings webpage and lecture webpage) Outline Speciation in irradiated fuel Utilization of
More informationFlow distribution and turbulent heat transfer in a hexagonal rod bundle experiment
Flow distribution and turbulent heat transfer in a hexagonal rod bundle experiment K. Litfin, A. Batta, A. G. Class,T. Wetzel, R. Stieglitz Karlsruhe Institute of Technology Institute for Nuclear and Energy
More informationDEMONSTRATION ACCELERATOR DRIVEN COMPLEX FOR EFFECTIVE INCINERATION OF 99 Tc AND 129 I
DEMONSTRATION ACCELERATOR DRIVEN COMPLEX FOR EFFECTIVE INCINERATION OF 99 Tc AND 129 I A.S. Gerasimov, G.V. Kiselev, L.A. Myrtsymova State Scientific Centre of the Russian Federation Institute of Theoretical
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationModification of PdH 2 and PdD 2 thin films processed by HeNe laser
Modification of PdH 2 and PdD 2 thin films processed by HeNe laser V.Nassisi #, G.Caretto #, A. Lorusso #, D.Manno %, L.Famà %, G.Buccolieri %, A.Buccolieri %, U.Mastromatteo* # Laboratory of Applied
More informationThermische Speicherung von Solarenergie
Thermische Speicherung von Solarenergie Dr. Thomas Bauer Institut für Technische Thermodynamik Stuttgart, Köln 15. Kölner Sonnenkolloquium, 12.6.2012 www.dlr.de/tt Slide 2 > 15. Kölner Sonnenkolloquium
More informationRESULTS OF R&D ON FUTURE FUEL CYCLE AND ASSOCIATED HL WASTE DISPOSAL: THE FRENCH CASE
IGDTP_SNETP_EF4, October 2930, 2013, Praha RESULTS OF R&D ON FUTURE FUEL CYCLE AND ASSOCIATED HL WASTE DISPOSAL: THE FRENCH CASE Dominique Warin CEA / Nuclear Energy Direction 29 OCTOBRE 2013 14 juin
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationIntroduction to Nuclear Fuel Cycle and Advanced Nuclear Fuels
Introduction to Nuclear Fuel Cycle and Advanced Nuclear Fuels Jon Carmack Deputy National Technical Director Fuel Cycle Technology Advanced Fuels Program February 27, 2011 The Evolution of Nuclear Power
More informationImproving regulatory practices through the OECDNEA Stress Corrosion Cracking and Cable Ageing Project (SCAP)
Improving regulatory practices through the OECDNEA Stress Corrosion Cracking and Cable Ageing Project (SCAP) A. Yamamoto a, A. Huerta a, K. Gott b, T. Koshy c a Nuclear Safety Division, OECD Nuclear Energy
More informationME349 Engineering Design Projects
ME349 Engineering Design Projects Introduction to Materials Selection The Material Selection Problem Design of an engineering component involves three interrelated problems: (i) selecting a material, (ii)
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationNotes on Polymer Rheology Outline
1 Why is rheology important? Examples of its importance Summary of important variables Description of the flow equations Flow regimes  laminar vs. turbulent  Reynolds number  definition of viscosity
More informationTENSILE AND CREEP DATA OF 316L (N) STAINLESS STEEL ANALYSIS
TENSILE AND CREEP DATA OF 316L (N) STAINLESS STEEL ANALYSIS V. Bindu Neeharika, K. S. Narayana, V. Krishna and M. Prasanth Kumar Mechanical Department, ANITS, Sangivalasa, Visakhapatnam India binduneeharika@yahoo.co.in
More informationTHREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL. Hossam Halfa
THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, hossamhalfa@cmrdi.sci.eg;
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationThermochemistry. Thermochemistry 1/25/2010. Reading: Chapter 5 (omit 5.8) As you read ask yourself
Thermochemistry Reading: Chapter 5 (omit 5.8) As you read ask yourself What is meant by the terms system and surroundings? How are they related to each other? How does energy get transferred between them?
More informationLecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows
Lecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows 3. 1 Basics: equations of continuum mechanics  balance equations for mass and momentum  balance equations for the energy and the chemical
More informationExergy: the quality of energy N. Woudstra
Exergy: the quality of energy N. Woudstra Introduction Characteristic for our society is a massive consumption of goods and energy. Continuation of this way of life in the long term is only possible if
More informationNorth American Stainless
North American Stainless Flat Products Stainless Steel Sheet T409 INTRODUCTION NAS 409 is an 11% chromium, stabilized ferritic stainless steel. It is not as resistant to corrosion or hightemperature oxidation
More informationCharacterization of Electronic Materials Using Thermal Analysis
application Note Thermal Analysis Characterization of Electronic Materials Using Thermal Analysis Thermal analysis comprises a series of powerful techniques for the characterization of the thermal, physical,
More informationLEADCOOLED FAST REACTOR (LFR) DEVELOPMENT GAPS
LEADCOOLED FAST REACTOR (LFR) DEVELOPMENT GAPS M. TARANTINO Italian National Agency for New Technologies, Energy and Sustainable Economic Development, C.R. ENEA Brasimone Italy mariano.tarantino@enea.it
More informationSCDAP/RELAP53D : A StateoftheArt Tool for Severe Accident Analyses
SCDAP/RELAP53D : A StateoftheArt Tool for Severe Accident Analyses D. L. Knudson and J. L. Rempe 2002 RELAP5 International Users Seminar Park City, Utah, USA September 46, 2002 Objective and Outline
More informationSafe ExploitAtion Related CHemistry for HLM reactors
SEARCH Safe ExploitAtion Related CHemistry for HLM reactors Paul Schuurmans for the SEARCH project Copyright 2012 SCK CEN International workshop on Innovative Nuclear Reactors cooled by Heavy Liquid Metals
More informationENERGY TRANSFER SYSTEMS AND THEIR DYNAMIC ANALYSIS
ENERGY TRANSFER SYSTEMS AND THEIR DYNAMIC ANALYSIS Many mechanical energy systems are devoted to transfer of energy between two points: the source or prime mover (input) and the load (output). For chemical
More informationFeasibility Analysis and Uncertainty Quantification for a "FastRunning" Chain of Codes for the NPP Accident Management
Agenzia nazionale per le nuove tecnologie, l energia e lo sviluppo economico sostenibile MINISTERO DEO SVIUPPO ECONOMICO Feasibility Analysis and Uncertainty Quantification for a "FastRunning" Chain of
More informationMaterial data sheet. EOS StainlessSteel GP1 for EOSINT M 270. Description, application
EOS StainlessSteel GP1 for EOSINT M 270 A number of different materials are available for use with EOSINT M systems, offering a broad range of emanufacturing applications. EOS StainlessSteel GP1 is a
More informationPolitecnico di Torino. Porto Institutional Repository
Politecnico di Torino Porto Institutional Repository [Other] Advanced highstrength steels for carbody manufacturing Original Citation: D. Firrao, G. Scavino, P. Matteis, M. De Sanctis, R. Valentini,
More informationProperties and Welding Procedure for Grade 91 Alloy Steel
International Journal of Engineering Research and Technology. ISSN 09743154 Volume 6, Number 6 (2013), pp. 767772 International Research Publication House http://www.irphouse.com Properties and Welding
More informationLaboratory scale electrical resistivity measurements to monitor the heat propagation within porous media for low enthalpy geothermal applications
32 CONVEGNO NAZIONALE 1921 Novembre 2013 TRIESTE Laboratory scale electrical resistivity measurements to monitor the heat propagation within porous media for low enthalpy geothermal applications N. Giordano
More informationa) Use the following equation from the lecture notes: = ( 8.314 J K 1 mol 1) ( ) 10 L
hermodynamics: Examples for chapter 4. 1. One mole of nitrogen gas is allowed to expand from 0.5 to 10 L reversible and isothermal process at 300 K. Calculate the change in molar entropy using a the ideal
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationProgress status of the FUTURIXFTA PIE programme for pins CEA7 & CEA8. F. Delage, G. Cécilia, J. Lamontagne, L. Loubet
Progress status of the FUTURIXFTA PIE programme for pins CEA7 & CEA8 F. Delage, G. Cécilia, J. Lamontagne, L. Loubet FAIRFUELS final workshop May 20, 2015 20/05/2015 CEA 10 AVRIL 2012 PAGE 1 He bonded
More informationTECHNICAL MEETING ON INPILE TESTING AND INSTRUMENTATION FOR DEVELOPMENT OF GENERATIONIV FUELS AND STRUCTURAL MATERIALS
651T1TM42785 TECHNICAL MEETING ON INPILE TESTING AND INSTRUMENTATION FOR DEVELOPMENT OF GENERATIONIV FUELS AND STRUCTURAL MATERIALS I. BACKGROUND Halden, Norway 21 24 August 2012 INFORMATION SHEET
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationAssessment of Correlations for Heat Transfer to the Coolant for Heavy Liquid Metal Cooled Core Designs
Forschungszentrum Karlsruhe in der HelmholtzGemeinschaft Wissenschaftliche Berichte FZKA 7352 Assessment of Correlations for Heat Transfer to the Coolant for Heavy Liquid Metal Cooled Core Designs W.
More informationStatus of the ALFRED Project. Alessandro Alemberti
Status of the ALFRED Project Alessandro Alemberti ESNII Biennial conference 171819 March 2015 Brussels Belgium 1 SUMMARY ALFRED AND FALCON ALFRED CONCEPTUAL DESIGN REVIEW ALFRED AND GENERATION IV ACTIVITIES
More informationk L a measurement in bioreactors
k L a measurement in bioreactors F. Scargiali, A. Busciglio, F. Grisafi, A. Brucato Dip. di Ingegneria Chimica, dei Processi e dei Materiali, Università di Palermo Viale delle Scienze, Ed. 6, 9018, Palermo,
More informationDESIGN, SAFETY AND FUEL DEVELOPMENTS FOR THE EFIT ACCELERATOR DRIVEN SYSTEM WITH CERCER AND CERMET CORES
DESIGN, SAFETY AND FUEL DEVELOPMENTS FOR THE EFIT ACCELERATOR DRIVEN SYSTEM WITH CERCER AND CERMET CORES W. Maschek 1, C. Artioli 2, X. Chen 1, F. Delage 3, A. FernandezCarretero 4, M. Flad 1, A. Fokau
More informationEsystem = 0 = Ein Eout
AGENDA: I. Introduction to Thermodynamics II. First Law Efficiency III. Second Law Efficiency IV. Property Diagrams and Power Cycles V. Additional Material, Terms, and Variables VI. Practice Problems I.
More informationA MTR FUEL ELEMENT FLOW DISTRIBUTION MEASUREMENT PRELIMINARY RESULTS
A MTR FUEL ELEMENT FLOW DISTRIBUTION MEASUREMENT PRELIMINARY RESULTS W. M. Torres, P. E. Umbehaun, D. A. Andrade and J. A. B. Souza Centro de Engenharia Nuclear Instituto de Pesquisas Energéticas e Nucleares
More informationENERGY. Thermochemistry. Heat. Temperature & Heat. Thermometers & Temperature. Temperature & Heat. Energy is the capacity to do work.
ENERGY Thermochemistry Energy is the capacity to do work. Chapter 6 Kinetic Energy thermal, mechanical, electrical, sound Potential Energy chemical, gravitational, electrostatic Heat Heat, or thermal energy,
More informationOn the neutronics of European leadcooled fast reactor
NUKLEONIKA 2010;55(3):317 322 ORIGINAL PAPER On the neutronics of European leadcooled fast reactor Jerzy Cetnar, Mikołaj Oettingen, Grażyna Domańska Abstract. The perspective of nuclear energy development
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationTHE IMPACT OF YIELD STRENGTH OF THE INTERCONNECTOR ON THE INTERNAL STRESS OF THE SOLAR CELL WITHIN A MODULE
5th World Conference on Photovoltaic Energy Conversion, 61 September 21, Valencia, Spain THE IMPACT OF YIELD STRENGTH OF THE INTERCONNECTOR ON THE INTERNAL STRESS OF THE SOLAR CELL WITHIN A MODULE Y.
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationBUMAX. REYHER your partner for the BUMAX range
BUMAX hightensile stainless steel fasteners REYHER your partner for the BUMAX range Strongest stainless steel fasteners in the world BUMAX 88 and BUMAX ready for delivery from stock Wide range of BUMAX
More information10 Nuclear Power Reactors Figure 10.1
10 Nuclear Power Reactors Figure 10.1 89 10.1 What is a Nuclear Power Station? The purpose of a power station is to generate electricity safely reliably and economically. Figure 10.1 is the schematic of
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationRevision of the DEMO core configuration and of its dynamic behaviour
Agenzia Nazionale per le Nuove Tecnologie, l Energia e lo Sviluppo Economico Sostenibile RICERCA DI SISTEMA EETTRICO Revision of the DEMO core configuration and of its dynamic behaviour G. Grasso, C. Petrovich
More informationApplied Thermodynamics for Marine Systems Prof. P. K. Das Department of Mechanical Engineering Indian Institute of Technology, Kharagpur
Applied Thermodynamics for Marine Systems Prof. P. K. Das Department of Mechanical Engineering Indian Institute of Technology, Kharagpur Lecture  7 Ideal Gas Laws, Different Processes Let us continue
More informationRef. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield
MTE 585 Oxidation of Materials Part 1 Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield Introduction To illustrate the case of high temperature oxidation, we will use Nibase superalloys.
More information10 Novembre 2011 ENEA  Via Giulio Romano 41, Roma
UNIVERSITÀ DI PISA GRUPPO DI RICERCA NUCLEARE SAN PIERO A GRADO (GRNSPG) Il reattore sperimentale per applicazioni scientifiche e industriali Novembre 2 ENEA  Via Giulio Romano 4, Roma Competenze ItalianeUtili
More informationIntegration of a fin experiment into the undergraduate heat transfer laboratory
Integration of a fin experiment into the undergraduate heat transfer laboratory H. I. AbuMulaweh Mechanical Engineering Department, Purdue University at Fort Wayne, Fort Wayne, IN 46805, USA Email: mulaweh@engr.ipfw.edu
More informationTENSILE TESTING PRACTICAL
TENSILE TESTING PRACTICAL MTK 2B Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in
More informationIndiana's Academic Standards 2010 ICP Indiana's Academic Standards 2016 ICP. map) that describe the relationship acceleration, velocity and distance.
.1.1 Measure the motion of objects to understand.1.1 Develop graphical, the relationships among distance, velocity and mathematical, and pictorial acceleration. Develop deeper understanding through representations
More informationV K Raina. Reactor Group, BARC
Critical facility for AHWR and PHWRs V K Raina Reactor Group, BARC India has large reserves of Thorium Critical facility Utilisation of Thorium for power production is a thrust area of the Indian Nuclear
More informationATI 2205 ATI 2205. Technical Data Sheet. Duplex Stainless Steel GENERAL PROPERTIES. (UNS S31803 and S32205)
ATI 2205 Duplex Stainless Steel (UNS S31803 and S32205) GENERAL PROPERTIES ATI 2205 alloy (UNS S31803 and/or S32205) is a nitrogenenhanced duplex stainless steel alloy. The nitrogen serves to significantly
More informationA NOVEL SINTERINGDISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS
Scripta mater. 44 (2001) 105 110 www.elsevier.com/locate/scriptamat A NOVEL SINTERINGDISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS Y.Y. Zhao and D.X. Sun Materials Science and Engineering, Department
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationSALT SPRAY AND IMMERSION CORROSION TESTING OF PM STAINLESS STEEL MATERIALS. W. Brian James Hoeganaes Corporation. Cinnaminson, NJ 08077
SALT SPRAY AND IMMERSION CORROSION TESTING OF PM STAINLESS STEEL MATERIALS W. Brian James Hoeganaes Corporation Cinnaminson, NJ 08077 Leander F. Pease III PowderTech Associates Inc. Andover, MA 01845
More informationDIPE: DETERMINATION OF INPUT PARAMETERS UNCERTAINTIES METHODOLOGY APPLIED TO CATHARE V2.5_1 THERMALHYDRAULICS CODE
5th International Conference on Nuclear Engineering Nagoya, Japan, April 2226, 27 ICONE5224 DIPE: DETERMINATION OF INPUT PARAMETERS UNCERTAINTIES METHODOLOGY APPLIED TO CATHARE V2.5_ THERMALHYDRAULICS
More informationRESULTS OF ICARUS 9 EXPERIMENTS RUN AT IMRA EUROPE
Roulette, T., J. Roulette, and S. Pons. Results of ICARUS 9 Experiments Run at IMRA Europe. in Sixth International Conference on Cold Fusion, Progress in New Hydrogen Energy. 1996. Lake Toya, Hokkaido,
More informationInvestigations of a LongDistance 1000 MW Heat Transport System with APROS Simulation Software
th International Conference on Structural Mechanics in Reactor Technology (SMiRT ) Espoo, Finland, August 94, 9 SMiRT Division 3, Paper 56 Investigations of a LongDistance MW Heat Transport System with
More informationChem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry
Chem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry Why? Chemists are concerned with mass relationships in chemical reactions, usually run on a macroscopic scale (grams, kilograms, etc.). To deal with
More informationChapter 8 Maxwell relations and measurable properties
Chapter 8 Maxwell relations and measurable properties 8.1 Maxwell relations Other thermodynamic potentials emerging from Legendre transforms allow us to switch independent variables and give rise to alternate
More informationCoupling Forced Convection in Air Gaps with Heat and Moisture Transfer inside Constructions
Coupling Forced Convection in Air Gaps with Heat and Moisture Transfer inside Constructions M. Bianchi Janetti 1, F. Ochs 1 and R. Pfluger 1 1 University of Innsbruck, Unit for Energy Efficient Buildings,
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationSOURCES OF RADIOACTIVITY
Section 10: FISSION POWER This section briefly describes the basic principles underlying the development of the fission power reactor, some examples of commercial reactors in use today and issues about
More informationEsystem = 0 = Ein Eout
AGENDA: I. Introduction to Thermodynamics II. First Law Efficiency III. Second Law Efficiency IV. Property Diagrams and Power Cycles V. Additional Material, Terms, and Variables VI. Practice Problems I.
More informationAPPLICATION OF TRANSIENT WELLBORE SIMULATOR TO EVALUATE DELIVERABILITY CURVE ON HYPOTHETICAL WELLX
PROCEEDINGS, ThirtyThird Workshop on Geothermal Reservoir Engineering Stanford University, Stanford, California, January 830, 008 SGPTR185 APPLICATION OF TRANSIENT WELLBORE SIMULATOR TO EVALUATE DELIVERABILITY
More informationAccidents of loss of flow for the ETTR2 reactor: deterministic analysis
NUKLEONIKA 2000;45(4):229 233 ORIGINAL PAPER Accidents of loss of flow for the ETTR2 reactor: deterministic analysis Ahmed Mohammed ElMessiry Abstract The main objective for reactor safety is to keep
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationCase Study: Fission Yield Module and the Oklo Nuclear Geyser
Radioactivity  Radionuclides  Radiation 8th MultiMedia Training Course with Nuclides.net (Institute Josžef Stefan, Ljubljana, 13 th 15 th September 2006) Thursday, 14 th September 2006 Case Study:
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationWe will try to get familiar with a heat pump, and try to determine its performance coefficient under different circumstances.
C4. Heat Pump I. OBJECTIVE OF THE EXPERIMENT We will try to get familiar with a heat pump, and try to determine its performance coefficient under different circumstances. II. INTRODUCTION II.1. Thermodynamic
More informationTadahiro Yasuda. Introduction. Overview of Criterion D200. Feature Article
F e a t u r e A r t i c l e Feature Article Development of a High Accuracy, Fast Response Mass Flow Module Utilizing Pressure Measurement with a Laminar Flow Element (Resistive Element) Criterion D200
More informationInternational Journal of Latest Research in Science and Technology Volume 4, Issue 2: Page No.161166, MarchApril 2015
International Journal of Latest Research in Science and Technology Volume 4, Issue 2: Page No.161166, MarchApril 2015 http://www.mnkjournals.com/ijlrst.htm ISSN (Online):22785299 EXPERIMENTAL STUDY
More informationChapter 18 Temperature, Heat, and the First Law of Thermodynamics. Problems: 8, 11, 13, 17, 21, 27, 29, 37, 39, 41, 47, 51, 57
Chapter 18 Temperature, Heat, and the First Law of Thermodynamics Problems: 8, 11, 13, 17, 21, 27, 29, 37, 39, 41, 47, 51, 57 Thermodynamics study and application of thermal energy temperature quantity
More informationA LAMINAR FLOW ELEMENT WITH A LINEAR PRESSURE DROP VERSUS VOLUMETRIC FLOW. 1998 ASME Fluids Engineering Division Summer Meeting
TELEDYNE HASTINGS TECHNICAL PAPERS INSTRUMENTS A LAMINAR FLOW ELEMENT WITH A LINEAR PRESSURE DROP VERSUS VOLUMETRIC FLOW Proceedings of FEDSM 98: June 5, 998, Washington, DC FEDSM98 49 ABSTRACT The pressure
More informationLASER MELTED STEEL FREE SURFACE FORMATION
METALLURGY AND FOUNDRY ENGINEERING Vol. 33, 2007, No. 1 Aleksander Siwek * LASER MELTED STEEL FREE SURFACE FORMATION 1. INTRODUCTION Many phisical phenomena happen on the surface of worked object in the
More informationBasic requirements 999GG01834
Basic requirements / DIVISIONE INGEGNERIA E INNOVAZIONE AREA DI BUSINESS SVILUPPO E REALIZZAZIONE IMPIANTI 1 Ince Sicurezza Security Index TITOLO Title Basic requirements for the Suppliers qualification
More informationFluids and Solids: Fundamentals
Fluids and Solids: Fundamentals We normally recognize three states of matter: solid; liquid and gas. However, liquid and gas are both fluids: in contrast to solids they lack the ability to resist deformation.
More informationNorth American Stainless
Introduction: North American Stainless Flat Products Stainless Steel Grade Sheet 309S (S30908)/ EN1.4833 SS309 is a highly alloyed austenitic stainless steel used for its excellent oxidation resistance,
More information